304 15 24MB
English Pages XXIII, 675  Year 2021
Science, Technology and Applications of Metal Additive Manufacturing provides a holistic picture of metal Additive Manuf
531 96 11MB Read more
Additive Manufacturing Technologies: Rapid Prototyping to Direct Digital Manufacturing deals with various aspects of joi
268 95 9MB Read more
This book provides a single-source reference to additive manufacturing, accessible to anyone with a basic background in
383 16 6MB Read more
This book serves as an accelerated learning tool for students of Additive Manufacturing. The author presents key aspects
292 108 14MB Read more
This book serves as an accelerated learning tool for students of Additive Manufacturing. The author presents key aspects
308 113 5MB Read more
In this book, basic sciences and applied technologies in 3D printing and 2D coating―including 2D surface modulations on
328 18 11MB Read more
This book contains the proceedings of the Additive Manufacturing in Product Development Conference. The content focus on
310 3 98MB Read more
Ian Gibson · David Rosen Brent Stucker · Mahyar Khorasani
Additive Manufacturing Technologies Third Edition
Additive Manufacturing Technologies
Ian Gibson • David Rosen • Brent Stucker Mahyar Khorasani
Additive Manufacturing Technologies Third Edition
Ian Gibson Department of Design, Production and Management University of Twente Enschede, The Netherlands
David Rosen George W. Woodruff School of Mechanical Engineering Georgia Institute of Technology Atlanta, GA, USA
Brent Stucker ANSYS Park City, UT, USA
Mahyar Khorasani Deakin University Armstrong Creek, VIC, Australia
ISBN 978-3-030-56126-0 ISBN 978-3-030-56127-7 (eBook) https://doi.org/10.1007/978-3-030-56127-7 © Springer Nature Switzerland AG 2021 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors, and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional affiliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland
Thank you for taking the time to read this textbook on Additive Manufacturing (AM). We hope you benefit from the time and effort it has taken putting it together and that you think it was a worthwhile undertaking. It all started as a discussion at a conference in Portugal when we realized we were putting together books with similar aims and objectives. Since we are friends as well as colleagues, it seemed sensible we join forces rather than compete; sharing the load and playing to each other’s strengths undoubtedly means a better all-round effort and result. We wrote this textbook because we have all been working in the field of AM for many years. Although none of us like to be called “old,” we do seem to have around 85 years of experience, collectively, and have each established reputations as educators and researchers in this field. We have each seen the technologies described in this textbook take shape and develop into serious commercial tools, with hundreds of thousands of regular users and many millions of parts being made by AM machines each year. AM is now being incorporated into curricula in many schools, polytechnics, and universities. More and more students are becoming aware of these technologies and yet, as we saw it, there was no single text adequate for such curricula. We believe that the first edition provided such a text, and based upon updated information, the 2nd and 3rd editions were developed. Additive Manufacturing includes a range of technologies that are capable of translating virtual solid model data into physical models in an automated process. The data are broken down into a series of 2D cross-sections of finite thickness. These cross-sections are fed into AM machines so that they can be created, combined, and added together in a layer-by-layer sequence to form the physical part. The geometry of the digital part is therefore reproduced physically in the AM machine without having to adjust for manufacturing processes, like attention to tooling, undercuts, draft angles, or other features. We can therefore say that the AM machine is a What You See Is What You Build (WYSIWYB) process that is particularly valuable the more complex the geometry. This basic principle drives nearly all AM machines, with variations in each technology in terms of the techniques used for creating layers and bonding them together. Further variations include speed, layer thickness, range of materials, accuracy, and, of course, cost. With so many v
variables, it is clear to see why this textbook must be so long and detailed. Having said that, we still feel there is much more we could have written. The first three chapters of this textbook provide a basic overview of AM processes. Without fully describing each technology, we provide an appreciation for why AM is so important to many branches of industry. We outline the rapid development of this technology from humble beginnings, which showed promise but still required much development, to one that is now maturing and showing a real benefit to product development organizations. By reading these chapters, we hope you can learn the basics of how AM works. The next eight chapters (Chaps. 4, 5, 6, 7, 8, 9, 10 and 11) take each group of technologies in turn and describe them in detail. The fundamentals of each technology are dealt with in terms of the basic process, whether it involves photopolymer curing, inkjet printing, sintering, melting, etc., so that the reader can appreciate what is needed in order to understand, develop, optimize, and use each technology. Most technologies discussed in this textbook have been commercialized by at least one company, and many of these commercial variants are described along with discussion on how to get the best out of them. The next two chapters are about hybrid AM (the mix of AM and other manufacturing processes in a single machine) and low-cost AM techniques. The low-cost AM chapter focuses on inexpensive machines, which overlaps some of the material in earlier chapters. However, we felt that the increasing interest in these low-cost machines justified the special treatment. The final nine chapters deal with how to apply AM technology in different settings. We look at the materials available for AM and the post-processing you need to perform after removing a part from the machine, before it can be used. We provide selection methods for sorting through the many machine options. Since all AM machines depend on input from 3D CAD software, we go on to discuss how software is used. We follow this with a discussion of novel applications which utilize AM machine output for end-product use, called Direct Digital Manufacturing. Many of these products were impossible, infeasible, or uneconomic in the past, including mass customization, where a product can be produced according to the tastes of an individual consumer but at a cost-effective price. Next we look at how AM affects the design process, considering how we might improve designs to take advantage of unique benefits of AM. This moves us on nicely to the subjects of applications of AM, including tooling and products in the medical, aerospace, and automotive sectors. We complete the textbook with a chapter on the business and societal implications of AM, investigating how AM enables creative businesses and entrepreneurs to invent new products. This textbook is primarily aimed at students and educators studying AM, either as a self-contained course or as a module within a larger course on manufacturing technology. There is sufficient depth for an undergraduate or graduate-level course, with many references to point the student further along the path. Each chapter also has a number of exercise questions designed to test the reader’s knowledge and to expand their thinking. A companion instructor’s guide is being developed as part of the 3rd edition. Researchers into AM may also find this text useful in helping them
understand the state of the art and the opportunities for further research. AM industry practitioners will also find this textbook useful as they guide their companies in adopting AM. We made a wide range of changes in moving from the first edition, completed in 2009, to the 2nd edition published in 2015. We added a number of new sections and chapters, including expanding the chapter on medical applications to include discussion on automotive and aerospace applications. A new chapter on rapid tooling was also added in the 2nd edition. Between the 1st and 2nd editions, the authors helped establish the ASTM F42 and ISO TC261 committees on Additive Manufacturing. These committees developed standard terminology for AM, and the 2nd edition used this updated terminology. In the 2nd edition, we also edited the text to reduce references to company-specific technologies and instead focused more on technological principles and general understanding. We split the original chapter on printing processes into two chapters on material jetting and on binder jetting to reflect the standard terminology and the evolution of these processes in different directions. We inserted a range of recent technological innovations, including discussion on the Additive Manufacturing File format. As a result of these many additions and changes, we believe the 2nd edition was significantly more comprehensive than the first. The response to this 2nd edition was positive, as sales increased by almost 40% 2 years after publishing, and by 2019 this book was firmly established as the leading AM textbook worldwide. To keep up with the extensive growth of AM since 2015, we decided to publish a 3rd edition. This took nearly 2 years of effort with a new co-author added to the list. Older examples of vat photopolymerization, material jetting, and binder jetting machines were replaced by newer technologies and applications. New variants of existing AM techniques, such as high-speed sintering, multi-material jetting, cold spray, friction stir AM, and more, were added to relevant chapters. We continue to update our materials to conform to international standards, including ASTM 52900 terminology. To help our readers understand how new terminology relates to older company-specific and technology-specific names, we have added information to Chaps. 5 and 10 cross-referencing nomenclature for AM processes to help address any confusion. Approximately 200 figures have been redrawn to improve understanding of the contents. We have significantly expanded our discussion of post-processing methods to improve surface quality, dimensional accuracy, and mechanical properties. We provide a better classification for different AM-related software. New topics like the influence of AM within Industry 4.0, design for 4D printing, and a discussion of design of experiments have also been added. Hybrid AM techniques and materials for AM have expanded dramatically since the 2nd edition, so we significantly expanded our treatment of these topics, resulting in two new chapters. Hybrid AM is a combination of additive and conventional manufacturing into a single process, resulting in significantly improved capabilities. In the new chapter on materials, we classify the feedstock based on the physical state of the material when added to the machine, including liquid, powder, and solid
states. This new chapter should help students, researchers, and professionals select a suitable machine/material combination for their research and businesses. We are currently working on online supplementary information for this textbook. In particular, we hope to publish a solutions manual soon. Please check online for its availability. Although we have worked hard to make this textbook as comprehensive as possible, we recognize that a textbook about such rapidly changing technology will not remain up-to-date for very long. If you have comments, questions, or suggestions for improvement, they are welcome. We anticipate updating this textbook in the future, and we look forward to hearing how you have used these materials and how we might improve this textbook. As mentioned earlier, each author is an established expert in AM with many years of research experience. In addition, in many ways, this textbook is only possible due to the many students and colleagues with whom we have collaborated over the years. To introduce you to the authors and some of the others who have made this textbook possible, we will end this preface with brief author acknowledgments. Enschede, The Netherlands Ian Gibson Atlanta, GA, USA David Rosen Park City, UT, USA Brent Stucker Armstrong Creek, VIC, Australia Mahyar Khorasani
Dr. Mahyar Khorasani, the newest member of our team, acknowledges Deakin University for providing time to edit this textbook. Without this cooperation as well as the support of his mentor, Professor Bernard Rolfe, the time-consuming editing process would not have been possible. Dr. Khorasani thanks his family, Giti, Massoud, and lovely Elmira, for their patience, encouragement, and love during the hours of writing and editing the contents and chapters. Dr. Khorasani would like to thank Amir Hossein Ghasemi for his great support and help in this edition. Prof. Brent Stucker thanks Utah State University, VTT Technical Research Center, and the University of Louisville for providing the academic freedom, sabbaticals, and environment needed to complete the 1st and 2nd editions and Ansys for providing support to complete the 3rd edition. This textbook would not have been possible without the many graduate students and postdoctoral researchers who have worked with Prof. Stucker over the years. In particular, he would like to thank Prof. G.D. Janaki Ram of the Indian Institute of Technology Hyderabad, whose co- authoring of the “Layer-Based Additive Manufacturing Technologies” chapter in the CRC Materials Processing Handbook helped lead to the organization of this textbook. Additionally, many students’ work directly led to content in this textbook and solution manual, including: Muni Malhotra, Xiuzhi Qu, Carson Esplin, Adam Smith, Joshua George, Christopher Robinson, Yanzhe Yang, Matthew Swank, John Obielodan, Kai Zeng, Haijun Gong, Xiaodong Xing, Hengfeng Gu, Md Anam, Nachiket Patil, and Deepankar Pal. Special thanks are due to Prof. Stucker’s wife, Gail, and their children, Tristie, Andrew, Megan, and Emma, who patiently supported many days and evenings on this textbook. Prof. Stucker has sought to merge his Christian faith with his work, and he hopes that this textbook inspires its readers to create amazing things that bring goodness to people around the world and, as a result, bring joy to God. Prof. David W. Rosen acknowledges support from Georgia Tech, the Singapore University of Technology and Design, and the many graduate students and postdocs who contributed technically to the content in this book. In particular, he thanks Drs. Fei Ding, Mahdi Emami, Amit Jariwala, Scott Johnston, Samyeon Kim, Ameya Limaye, J. Mark Meacham, Sang-In Park, Benay Sager, L. Angela Tse, Hongqing ix
Wang, Chris Williams, Yong Yang, Xiong Yi, Xiayun Zhao, and Wenchao Zhou as well as Lauren Margolin. He also appreciates the many students who took his graduate-level course at Georgia Tech for their feedback on the textbook and their project ideas. Special thanks goes out to his wife Joan and children Erik and Krista for their patience while he worked on this book. Prof. Ian Gibson would like to acknowledge the support of the Fraunhofer Project Center at the University of Twente and Deakin University in providing sufficient time for him to work on this book. He sincerely wishes to thank his lovely wife, Lina, for her patience, love, and understanding during the long hours preparing the material and writing the chapters. He also dedicates this textbook to his parents, June Gibson and Robert Ervin Gibson, as well as his children, Louise, Claire, and James. He hopes they would be proud of this wonderful achievement.
1 Introduction and Basic Principles���������������������������������������������������������� 1 1.1 What Is Additive Manufacturing?���������������������������������������������������� 1 1.2 What Are AM Parts Used For? �������������������������������������������������������� 3 1.3 The Generic AM Process������������������������������������������������������������������ 3 1.3.1 Step 1: CAD�������������������������������������������������������������������������� 4 1.3.2 Step 2: Conversion to STL���������������������������������������������������� 5 1.3.3 Step 3: Transfer to AM Machine and STL File Manipulation ������������������������������������������������������������������������ 5 1.3.4 Step 4: Machine Setup���������������������������������������������������������� 5 1.3.5 Step 5: Build�������������������������������������������������������������������������� 5 1.3.6 Step 6: Removal�������������������������������������������������������������������� 5 1.3.7 Step 7: Post-Processing �������������������������������������������������������� 6 1.3.8 Step 8: Application���������������������������������������������������������������� 6 1.4 Why Use the Term Additive Manufacturing? ���������������������������������� 6 1.4.1 Automated Fabrication (Autofab) ���������������������������������������� 7 1.4.2 Freeform Fabrication or Solid Freeform Fabrication������������ 7 1.4.3 Additive Manufacturing or Layer-Based Manufacturing ���������������������������������������������������������������������� 7 1.4.4 Rapid Prototyping ���������������������������������������������������������������� 8 1.4.5 Stereolithography or 3D Printing������������������������������������������ 8 1.5 The Benefits of AM�������������������������������������������������������������������������� 9 1.6 Distinction Between AM and Conventional Manufacturing Processes ������������������������������������������������������������������������������������������ 10 1.6.1 Material �������������������������������������������������������������������������������� 10 1.6.2 Speed ������������������������������������������������������������������������������������ 10 1.6.3 Complexity���������������������������������������������������������������������������� 11 1.6.4 Accuracy ������������������������������������������������������������������������������ 11 1.6.5 Geometry������������������������������������������������������������������������������ 12 1.6.6 Programming������������������������������������������������������������������������ 12 1.7 Example AM Parts���������������������������������������������������������������������������� 13
1.8 Other Related Technologies�������������������������������������������������������������� 14 1.8.1 Reverse Engineering Technology������������������������������������������ 14 1.8.2 Computer-Aided Engineering/Technologies (CAX)������������ 15 1.8.3 Haptic-Based CAD��������������������������������������������������������������� 16 1.9 About This Book������������������������������������������������������������������������������ 18 1.10 Questions������������������������������������������������������������������������������������������ 19 References�������������������������������������������������������������������������������������������������� 21 2 Development of Additive Manufacturing Technology�������������������������� 23 2.1 Introduction�������������������������������������������������������������������������������������� 23 2.2 Computers ���������������������������������������������������������������������������������������� 24 2.3 Computer-Aided Design Technology ���������������������������������������������� 26 2.4 Other Associated Technologies�������������������������������������������������������� 30 2.4.1 Printing Technologies������������������������������������������������������������ 30 2.4.2 Programmable Logic Controllers������������������������������������������ 31 2.4.3 Materials�������������������������������������������������������������������������������� 31 2.4.4 Computer Numerically Controlled Machining �������������������� 31 2.5 The Use of Layers���������������������������������������������������������������������������� 32 2.6 Classification of AM Processes�������������������������������������������������������� 33 2.6.1 Liquid Polymer Systems ������������������������������������������������������ 35 2.6.2 Discrete Particle Systems������������������������������������������������������ 35 2.6.3 Molten Material Systems������������������������������������������������������ 36 2.6.4 Solid Sheet Systems�������������������������������������������������������������� 37 2.6.5 New AM Classification Schemes������������������������������������������ 38 2.7 Heat Sources ������������������������������������������������������������������������������������ 39 2.7.1 Lasers������������������������������������������������������������������������������������ 39 2.7.2 Electron Beam���������������������������������������������������������������������� 41 2.7.3 Electric Arc/Plasma Arc�������������������������������������������������������� 41 2.8 Metal Systems���������������������������������������������������������������������������������� 42 2.9 Hybrid Systems�������������������������������������������������������������������������������� 42 2.10 Milestones in AM Development ������������������������������������������������������ 43 2.11 AM around the World ���������������������������������������������������������������������� 45 2.12 AM Standards ���������������������������������������������������������������������������������� 47 2.13 The Future? Rapid Prototyping Develops into Direct Digital Manufacturing���������������������������������������������������������������������������������� 48 2.14 Questions������������������������������������������������������������������������������������������ 49 References�������������������������������������������������������������������������������������������������� 50 3 Generalized Additive Manufacturing Process Chain �������������������������� 53 3.1 Introduction�������������������������������������������������������������������������������������� 53 3.2 The Eight Steps in Additive Manufacture���������������������������������������� 54 3.2.1 Step 1: Conceptualization and CAD ������������������������������������ 54 3.2.2 Step 2: Conversion to STL/AMF������������������������������������������ 56 3.2.3 Step 3: Transfer to AM Machine and STL File Manipulation ������������������������������������������������������������������������ 57 3.2.4 Step 4: Machine Setup���������������������������������������������������������� 58
3.2.5 Step 5: Build�������������������������������������������������������������������������� 58 3.2.6 Step 6: Removal and Cleanup ���������������������������������������������� 59 3.2.7 Step 7: Post-processing �������������������������������������������������������� 59 3.2.8 Step 8: Application���������������������������������������������������������������� 60 3.3 Variations from One AM Machine to Another���������������������������������� 60 3.3.1 Photopolymer-Based Systems���������������������������������������������� 61 3.3.2 Powder-Based Systems �������������������������������������������������������� 62 3.3.3 Molten Material Systems������������������������������������������������������ 62 3.3.4 Solid Sheets�������������������������������������������������������������������������� 63 3.4 Metal Systems���������������������������������������������������������������������������������� 63 3.4.1 The Use of Substrates����������������������������������������������������������� 63 3.4.2 Energy Density���������������������������������������������������������������������� 64 3.4.3 Weight ���������������������������������������������������������������������������������� 64 3.4.4 Accuracy ������������������������������������������������������������������������������ 65 3.4.5 Speed ������������������������������������������������������������������������������������ 65 3.4.6 Build Rate����������������������������������������������������������������������������� 66 3.5 Maintenance of Equipment �������������������������������������������������������������� 66 3.6 Materials Handling Issues���������������������������������������������������������������� 66 3.7 Design for AM���������������������������������������������������������������������������������� 68 3.7.1 Part Orientation �������������������������������������������������������������������� 68 3.7.2 Removal of Supports������������������������������������������������������������ 69 3.7.3 Hollowing Out Parts�������������������������������������������������������������� 69 3.7.4 Inclusion of Undercuts and Other Manufacturing Constraining Features����������������������������������������������������������� 69 3.7.5 Interlocking Features������������������������������������������������������������ 70 3.7.6 Reduction of Part Count in an Assembly������������������������������ 71 3.7.7 Identification Markings/Numbers ���������������������������������������� 71 3.8 Application Areas for AM-Enabled Product Development�������������� 71 3.8.1 Medical Modeling ���������������������������������������������������������������� 72 3.8.2 Reverse Engineering Data���������������������������������������������������� 72 3.8.3 Architectural Modeling �������������������������������������������������������� 72 3.8.4 Automotive���������������������������������������������������������������������������� 72 3.8.5 Aerospace������������������������������������������������������������������������������ 73 3.9 Further Discussion���������������������������������������������������������������������������� 73 3.10 Questions������������������������������������������������������������������������������������������ 74 References�������������������������������������������������������������������������������������������������� 75 4 Vat Photopolymerization������������������������������������������������������������������������ 77 4.1 Introduction�������������������������������������������������������������������������������������� 77 4.2 Vat Photopolymerization Materials�������������������������������������������������� 79 4.2.1 UV Curable Photopolymers�������������������������������������������������� 79 4.2.2 Overview of Photopolymer Chemistry �������������������������������� 81 4.2.3 Resin Formulations and Reaction Mechanisms�������������������� 83 4.3 Reaction Rates���������������������������������������������������������������������������������� 87 4.4 Laser Scan Vat Photopolymerization������������������������������������������������ 87
4.5 Photopolymerization Process Modeling ������������������������������������������ 88 4.5.1 Irradiance and Exposure�������������������������������������������������������� 89 4.5.2 Laser–Resin Interaction�������������������������������������������������������� 91 4.5.3 Photospeed���������������������������������������������������������������������������� 94 4.5.4 Time Scales �������������������������������������������������������������������������� 95 4.6 Vector Scan VPP Machines�������������������������������������������������������������� 96 4.7 Scan Patterns������������������������������������������������������������������������������������ 98 4.7.1 Layer-Based Build Phenomena and Errors �������������������������� 98 4.7.2 Weave������������������������������������������������������������������������������������ 100 4.7.3 Star-Weave���������������������������������������������������������������������������� 101 4.7.4 ACES Scan Pattern���������������������������������������������������������������� 103 4.8 Vector Scan Micro Vat Photopolymerization������������������������������������ 107 4.9 Mask Projection VPP Technologies and Processes�������������������������� 108 4.9.1 Mask Projection VPP Technology���������������������������������������� 108 4.9.2 Commercial MPVPP Systems���������������������������������������������� 110 4.9.3 MPVPP Modeling ���������������������������������������������������������������� 111 4.9.4 Continuous Liquid Interface Production (CLIP) Technology���������������������������������������������������������������������������� 113 4.10 Two-Photon Vat Photopolymerization���������������������������������������������� 113 4.11 Process Benefits and Drawbacks������������������������������������������������������ 115 4.12 Summary ������������������������������������������������������������������������������������������ 116 4.13 Questions������������������������������������������������������������������������������������������ 117 References�������������������������������������������������������������������������������������������������� 121 5 Powder Bed Fusion���������������������������������������������������������������������������������� 125 5.1 Introduction�������������������������������������������������������������������������������������� 125 5.2 Materials ������������������������������������������������������������������������������������������ 127 5.2.1 Polymers and Composites ���������������������������������������������������� 127 5.2.2 Metals and Composites �������������������������������������������������������� 128 5.2.3 Ceramics and Ceramic Composites�������������������������������������� 130 5.3 Powder Fusion Mechanisms ������������������������������������������������������������ 130 5.3.1 Solid-State Sintering ������������������������������������������������������������ 131 5.3.2 Chemically Induced Sintering���������������������������������������������� 134 5.3.3 Liquid-Phase Sintering and Partial Melting�������������������������� 134 5.3.4 Full Melting�������������������������������������������������������������������������� 138 5.3.5 High-Speed Sintering������������������������������������������������������������ 139 5.4 Metal and Ceramic Part Fabrication ������������������������������������������������ 141 5.4.1 Metal Parts���������������������������������������������������������������������������� 141 5.4.2 Ceramic Parts������������������������������������������������������������������������ 142 5.5 Process Parameters and Analysis������������������������������������������������������ 143 5.5.1 Process Parameters���������������������������������������������������������������� 143 5.5.2 Applied Energy Correlations and Scan Patterns ������������������ 145 5.6 Powder Handling������������������������������������������������������������������������������ 149 5.6.1 Powder Handling Challenges������������������������������������������������ 149 5.6.2 Powder Handling Systems���������������������������������������������������� 150 5.6.3 Powder Recycling ���������������������������������������������������������������� 152
5.7 Powder Bed Fusion Process Variants and Commercial Machines ������������������������������������������������������������������������������������������ 153 5.7.1 Polymer Laser Sintering (pLS) �������������������������������������������� 153 5.7.2 Laser-Based Systems for Metals and Ceramics�������������������� 156 5.7.3 Electron Beam Powder Bed Fusion�������������������������������������� 159 5.7.4 Line-Wise and Layer-Wise PBF Processes for Polymers�������������������������������������������������������������������������������� 163 5.8 Process Benefits and Drawbacks������������������������������������������������������ 165 5.9 Summary ������������������������������������������������������������������������������������������ 167 5.10 Questions������������������������������������������������������������������������������������������ 167 References�������������������������������������������������������������������������������������������������� 169 6 Material Extrusion���������������������������������������������������������������������������������� 171 6.1 Introduction�������������������������������������������������������������������������������������� 171 6.2 Basic Principles�������������������������������������������������������������������������������� 172 6.2.1 Material Loading������������������������������������������������������������������ 173 6.2.2 Liquification�������������������������������������������������������������������������� 173 6.2.3 Extrusion ������������������������������������������������������������������������������ 174 6.2.4 Solidification ������������������������������������������������������������������������ 176 6.2.5 Positional Control����������������������������������������������������������������� 176 6.2.6 Bonding �������������������������������������������������������������������������������� 178 6.2.7 Support Generation �������������������������������������������������������������� 179 6.3 Plotting and Path Control������������������������������������������������������������������ 180 6.4 Material Extrusion Machine Types �������������������������������������������������� 183 6.4.1 MEX Machines from Stratasys �������������������������������������������� 184 6.4.2 Other Material Extrusion Machines�������������������������������������� 186 6.4.3 Pellet-Fed Machines�������������������������������������������������������������� 187 6.5 Materials ������������������������������������������������������������������������������������������ 188 6.6 Limitations of MEX�������������������������������������������������������������������������� 192 6.7 Bioextrusion�������������������������������������������������������������������������������������� 193 6.7.1 Gel Formation ���������������������������������������������������������������������� 193 6.7.2 Melt Extrusion���������������������������������������������������������������������� 194 6.7.3 Scaffold Architectures ���������������������������������������������������������� 195 6.8 Other Systems ���������������������������������������������������������������������������������� 196 6.8.1 Contour Crafting ������������������������������������������������������������������ 196 6.8.2 Nonplanar Systems��������������������������������������������������������������� 196 6.8.3 Material Extrusion of Ceramics�������������������������������������������� 197 6.8.4 RepRap and [email protected]������������������������������������������������������ 198 6.9 Questions������������������������������������������������������������������������������������������ 199 References�������������������������������������������������������������������������������������������������� 200 7 Material Jetting���������������������������������������������������������������������������������������� 203 7.1 Evolution of Printing as an Additive Manufacturing Process���������� 204 7.2 Materials for Material Jetting������������������������������������������������������������ 205 7.2.1 Polymers�������������������������������������������������������������������������������� 205 7.2.2 Ceramics�������������������������������������������������������������������������������� 208
7.2.3 Metals������������������������������������������������������������������������������������ 210 7.2.4 Solution- and Dispersion-Based Deposition ������������������������ 211 7.3 Material Processing Fundamentals �������������������������������������������������� 212 7.3.1 Technical Challenges of MJT������������������������������������������������ 212 7.3.2 Droplet Formation Technologies������������������������������������������ 214 7.3.3 Continuous Mode������������������������������������������������������������������ 215 7.3.4 Drop-on-Demand Mode�������������������������������������������������������� 217 7.3.5 Other Droplet Formation Methods���������������������������������������� 218 7.4 Cold Spray���������������������������������������������������������������������������������������� 220 7.5 MJT Process Modeling �������������������������������������������������������������������� 220 7.6 Material Jetting Machines���������������������������������������������������������������� 226 7.7 Process Parameters in Material Jetting �������������������������������������������� 227 7.8 Rotative Material Jetting������������������������������������������������������������������ 228 7.9 Process Benefits and Drawbacks������������������������������������������������������ 229 7.10 Summary ������������������������������������������������������������������������������������������ 230 7.11 Questions������������������������������������������������������������������������������������������ 231 References�������������������������������������������������������������������������������������������������� 233 8 Binder Jetting ������������������������������������������������������������������������������������������ 237 8.1 Introduction�������������������������������������������������������������������������������������� 237 8.2 Materials ������������������������������������������������������������������������������������������ 239 8.2.1 Commercially Available Materials���������������������������������������� 239 8.2.2 Metal and Ceramic Materials Research�������������������������������� 241 8.3 Process Variations ���������������������������������������������������������������������������� 242 8.4 BJT Machines ���������������������������������������������������������������������������������� 245 8.5 Process Benefits and Drawbacks������������������������������������������������������ 248 8.6 Summary ������������������������������������������������������������������������������������������ 250 8.7 Questions������������������������������������������������������������������������������������������ 251 References�������������������������������������������������������������������������������������������������� 252 9 Sheet Lamination ������������������������������������������������������������������������������������ 253 9.1 Introduction�������������������������������������������������������������������������������������� 253 9.1.1 Gluing or Adhesive Bonding������������������������������������������������ 254 9.1.2 Bond-then-Form Processes �������������������������������������������������� 254 9.1.3 Form-then-Bond Processes �������������������������������������������������� 256 9.2 Materials ������������������������������������������������������������������������������������������ 259 9.3 Material Processing Fundamentals �������������������������������������������������� 260 9.3.1 Thermal Bonding������������������������������������������������������������������ 260 9.3.2 Sheet Metal Clamping���������������������������������������������������������� 261 9.4 Ultrasonic Additive Manufacturing�������������������������������������������������� 262 9.4.1 UAM Bond Quality�������������������������������������������������������������� 265 9.4.2 UAM Process Fundamentals������������������������������������������������ 266 9.4.3 UAM Process Parameters and Process Optimization����������� 267 9.4.4 Microstructures and Mechanical Properties of UAM Parts���������������������������������������������������������������������������� 270 9.4.5 UAM Applications���������������������������������������������������������������� 273
9.5 Sheet Lamination Benefits and Drawbacks�������������������������������������� 279 9.6 Commercial Trends�������������������������������������������������������������������������� 280 9.7 Summary ������������������������������������������������������������������������������������������ 280 9.8 Questions������������������������������������������������������������������������������������������ 281 References�������������������������������������������������������������������������������������������������� 282 10 Directed Energy Deposition�������������������������������������������������������������������� 285 10.1 Introduction������������������������������������������������������������������������������������ 285 10.2 General Directed Energy Deposition Process Description ������������ 287 10.3 Material Delivery���������������������������������������������������������������������������� 289 10.3.1 Powder Feeding���������������������������������������������������������������� 289 10.3.2 Wire Feeding�������������������������������������������������������������������� 292 10.4 DED Systems���������������������������������������������������������������������������������� 292 10.4.1 Laser Powder Deposition Processes �������������������������������� 293 10.4.2 Electron Beam Based Metal Deposition Processes���������� 298 10.4.3 Wire Arc Additive Manufacturing (WAAM)�������������������� 301 10.4.4 Friction Stir Additive Manufacturing (FSAM) ���������������� 303 10.4.5 Other DED Materials and Processes�������������������������������� 305 10.5 Process Parameters�������������������������������������������������������������������������� 305 10.6 Typical Materials and Microstructure �������������������������������������������� 306 10.7 Processing–Structure–Properties Relationships������������������������������ 309 10.8 DED Benefits and Drawbacks�������������������������������������������������������� 314 10.9 Questions���������������������������������������������������������������������������������������� 316 References�������������������������������������������������������������������������������������������������� 317 11 Direct Write Technologies ���������������������������������������������������������������������� 319 11.1 Direct Write Technologies�������������������������������������������������������������� 319 11.2 Background ������������������������������������������������������������������������������������ 320 11.3 Materials in Direct Write Technology�������������������������������������������� 320 11.4 Ink-Based DW�������������������������������������������������������������������������������� 321 11.5 Nozzle Dispensing Processes���������������������������������������������������������� 323 11.5.1 Quill-Type Processes�������������������������������������������������������� 324 11.5.2 Inkjet Printing Processes�������������������������������������������������� 326 11.5.3 Aerosol DW���������������������������������������������������������������������� 326 11.6 Laser Transfer DW�������������������������������������������������������������������������� 328 11.7 Thermal Spray DW ������������������������������������������������������������������������ 331 11.8 Electroforming�������������������������������������������������������������������������������� 333 11.9 Beam Deposition DW �������������������������������������������������������������������� 334 11.9.1 Laser CVD������������������������������������������������������������������������ 334 11.9.2 Focused Ion Beam CVD �������������������������������������������������� 336 11.9.3 Electron Beam CVD �������������������������������������������������������� 337 11.10 Liquid-Phase Deposition���������������������������������������������������������������� 337 11.11 Beam Tracing Approaches to Additive/Subtractive DW���������������� 338 11.11.1 Electron Beam Tracing ���������������������������������������������������� 338 11.11.2 Focused Ion Beam Tracing ���������������������������������������������� 339 11.11.3 Laser Beam Tracing���������������������������������������������������������� 339
11.12 Hybrid Direct Write Technologies�������������������������������������������������� 340 11.13 Applications of Direct Write���������������������������������������������������������� 340 11.14 Technical Challenges in Direct Write �������������������������������������������� 342 11.15 Questions���������������������������������������������������������������������������������������� 343 References�������������������������������������������������������������������������������������������������� 344 12 Hybrid Additive Manufacturing������������������������������������������������������������ 347 12.1 Hybrid Manufacturing�������������������������������������������������������������������� 347 12.2 Hybrid Manufacturing Processes���������������������������������������������������� 348 12.3 Hybrid Additive Manufacturing Principles������������������������������������ 351 12.3.1 Inseparable Hybrid Processes ������������������������������������������ 351 12.3.2 Synergy in Hybrid AM������������������������������������������������������ 351 12.3.3 Hybrid Materials �������������������������������������������������������������� 351 12.3.4 Part Quality and Process Efficiency���������������������������������� 352 12.4 Sequential Hybrid AM Classification Based on Secondary Processes ���������������������������������������������������������������������������������������� 352 12.4.1 Hybrid AM by Machining������������������������������������������������ 353 12.4.2 Hybrid AM by Rolling������������������������������������������������������ 355 12.4.3 Hybrid AM by Burnishing������������������������������������������������ 356 12.4.4 Hybrid AM by Friction Stir Processing���������������������������� 356 12.4.5 Hybrid AM by Ablation or Erosion���������������������������������� 357 12.4.6 Hybrid AM by Peening ���������������������������������������������������� 357 12.4.7 Hybrid AM by Pulsed Laser Deposition�������������������������� 360 12.4.8 Hybrid AM by Remelting ������������������������������������������������ 361 12.4.9 Hybrid AM by Laser-Assisted Plasma Deposition ���������� 362 12.5 Summary ���������������������������������������������������������������������������������������� 362 12.6 Questions���������������������������������������������������������������������������������������� 363 References�������������������������������������������������������������������������������������������������� 364 13 The Impact of Low-Cost AM Systems �������������������������������������������������� 367 13.1 Introduction������������������������������������������������������������������������������������ 367 13.2 Intellectual Property������������������������������������������������������������������������ 368 13.3 Disruptive Innovation���������������������������������������������������������������������� 370 13.3.1 Disruptive Business Opportunities������������������������������������ 370 13.3.2 Media Attention���������������������������������������������������������������� 371 13.4 The Maker Movement�������������������������������������������������������������������� 374 13.5 The Future of Low-Cost AM���������������������������������������������������������� 376 13.6 Questions���������������������������������������������������������������������������������������� 376 References�������������������������������������������������������������������������������������������������� 377 14 Materials for Additive Manufacturing�������������������������������������������������� 379 14.1 Introduction������������������������������������������������������������������������������������ 379 14.2 Feedstock for AM Processes���������������������������������������������������������� 381 14.3 Liquid-Based Material�������������������������������������������������������������������� 383 14.3.1 Liquids for VPP���������������������������������������������������������������� 387 14.3.2 Liquid Polymer Material for MJT and BJT���������������������� 388
14.3.3 Liquid Metal Material for MJT���������������������������������������� 390 14.3.4 Liquid Ceramic Composite Materials for VPP and MJT���������������������������������������������������������������������������� 390 14.3.5 Support Material �������������������������������������������������������������� 392 14.3.6 Other Liquid Polymer Feedstock�������������������������������������� 392 14.4 Powder-Based Materials ���������������������������������������������������������������� 392 14.4.1 Polymer Powder Material ������������������������������������������������ 393 14.4.2 Metal Powder Material for PBF, DED, and BJT�������������� 394 14.4.3 Ceramic Powder Material ������������������������������������������������ 399 14.4.4 Composite Powder for AM Processes������������������������������ 402 14.5 Solid-Based Materials�������������������������������������������������������������������� 405 14.5.1 Solid Polymer Feedstock for MEX���������������������������������� 405 14.5.2 Solid Metal Feedstock for DED and MEX SHL�������������� 408 14.5.3 Solid Ceramic Feedstock for SHL and MEX ������������������ 413 14.5.4 Solid-Based Composite Materials for SHL, MEX, and DED��������������������������������������������������������������������������� 415 14.6 Material Issues in AM�������������������������������������������������������������������� 420 14.6.1 Build Orientation�������������������������������������������������������������� 420 14.6.2 Keyholes���������������������������������������������������������������������������� 421 14.6.3 Chemical Degradation and Oxidation������������������������������ 421 14.6.4 Reactive Processes������������������������������������������������������������ 421 14.6.5 Assistive Gas and Residual Particles�������������������������������� 421 14.6.6 Cracks ������������������������������������������������������������������������������ 422 14.6.7 Delamination�������������������������������������������������������������������� 422 14.6.8 Distortion�������������������������������������������������������������������������� 422 14.6.9 Inclusions�������������������������������������������������������������������������� 423 14.6.10 Poor Surface Finish���������������������������������������������������������� 423 14.6.11 Porosity ���������������������������������������������������������������������������� 423 14.6.12 Shelf Life or Lifetime of the Feedstock���������������������������� 423 14.6.13 Support Structures������������������������������������������������������������ 424 14.7 Questions���������������������������������������������������������������������������������������� 424 References�������������������������������������������������������������������������������������������������� 425 15 Guidelines for Process Selection ������������������������������������������������������������ 429 15.1 Introduction������������������������������������������������������������������������������������ 429 15.2 Selection Methods for a Part���������������������������������������������������������� 430 15.2.1 Decision Theory���������������������������������������������������������������� 430 15.2.2 Approaches to Determining Feasibility���������������������������� 431 15.2.3 Approaches to Selection �������������������������������������������������� 433 15.2.4 Selection Example������������������������������������������������������������ 436 15.3 Challenges of Selection������������������������������������������������������������������ 438 15.4 Example System for Preliminary Selection������������������������������������ 442 15.5 Production Planning and Control���������������������������������������������������� 448 15.5.1 Production Planning���������������������������������������������������������� 449 15.5.2 Pre-Processing������������������������������������������������������������������ 449
15.5.3 Part Build Time ���������������������������������������������������������������� 451 15.5.4 Post-Processing ���������������������������������������������������������������� 452 15.5.5 Summary �������������������������������������������������������������������������� 452 15.6 Future Work������������������������������������������������������������������������������������ 453 15.7 Questions���������������������������������������������������������������������������������������� 454 References�������������������������������������������������������������������������������������������������� 455
16 Post-Processing���������������������������������������������������������������������������������������� 457 16.1 Introduction������������������������������������������������������������������������������������ 457 16.2 Post-Processing to Improve Surface Quality���������������������������������� 458 16.2.1 Support Material Removal������������������������������������������������ 458 16.2.2 Surface Texture Improvements ���������������������������������������� 462 16.2.3 Aesthetic Improvements �������������������������������������������������� 463 16.3 Post-Processing to Improve Dimensional Deviations�������������������� 464 16.3.1 Accuracy Improvements �������������������������������������������������� 464 16.3.2 Sources of Inaccuracy ������������������������������������������������������ 464 16.3.3 Model Pre-Processing to Compensate for Inaccuracy ������������������������������������������������������������������������ 465 16.3.4 Machining Strategy���������������������������������������������������������� 466 16.4 Post-Processing to Improve Mechanical Properties������������������������ 476 16.4.1 Property Enhancements Using Nonthermal Techniques������������������������������������������������������������������������ 476 16.4.2 Property Enhancements Using Thermal Techniques�������� 478 16.5 Preparation for Use as a Pattern������������������������������������������������������ 482 16.5.1 Investment Casting Patterns���������������������������������������������� 483 16.5.2 Sand Casting Patterns ������������������������������������������������������ 484 16.5.3 Other Pattern Replication Methods���������������������������������� 485 16.6 Summary ���������������������������������������������������������������������������������������� 486 16.7 Questions���������������������������������������������������������������������������������������� 487 References�������������������������������������������������������������������������������������������������� 487 17 Software for Additive Manufacturing���������������������������������������������������� 491 17.1 Introduction������������������������������������������������������������������������������������ 491 17.2 AM Software for STL Editing�������������������������������������������������������� 492 17.2.1 Preparation of CAD Models: The STL File���������������������� 493 17.3 AM Software for Slicing���������������������������������������������������������������� 497 17.3.1 Calculation of Each Slice Profile�������������������������������������� 498 17.3.2 Technology-Specific Elements������������������������������������������ 502 17.4 AM Software for STL Manipulation���������������������������������������������� 504 17.4.1 STL File Manipulation������������������������������������������������������ 505 17.4.2 Mesh Healing�������������������������������������������������������������������� 507 17.4.3 Surface Offsetting ������������������������������������������������������������ 507 17.4.4 STL Manipulation on the AM Machine���������������������������� 508 17.5 Problems with STL Files���������������������������������������������������������������� 508
17.6 Beyond the STL File���������������������������������������������������������������������� 511 17.6.1 Direct Slicing of the CAD Model ������������������������������������ 511 17.6.2 Color Models�������������������������������������������������������������������� 512 17.6.3 Multiple Materials������������������������������������������������������������ 512 17.6.4 Use of STL for Machining������������������������������������������������ 512 17.7 AM Software for Process Visualization and Collision Detection ���������������������������������������������������������������������������������������� 513 17.8 AM Software for Topology Optimization�������������������������������������� 514 17.9 AM Software for Modeling and Simulation ���������������������������������� 516 17.10 Manufacturing Execution System Software for AM���������������������� 518 17.11 The Additive Manufacturing File (AMF) Format�������������������������� 520 17.12 Questions���������������������������������������������������������������������������������������� 522 References�������������������������������������������������������������������������������������������������� 522 18 Direct Digital Manufacturing ���������������������������������������������������������������� 525 18.1 Introduction������������������������������������������������������������������������������������ 525 18.2 Early DDM Examples�������������������������������������������������������������������� 526 18.2.1 Align Technology�������������������������������������������������������������� 527 18.2.2 Siemens and Phonak �������������������������������������������������������� 528 18.2.3 Polymer Aerospace Parts�������������������������������������������������� 530 18.3 Applications of DDM �������������������������������������������������������������������� 531 18.3.1 Aerospace and Power Generation Industries�������������������� 532 18.3.2 Automotive Industry �������������������������������������������������������� 534 18.3.3 Medical Industry �������������������������������������������������������������� 535 18.3.4 Consumer Industries �������������������������������������������������������� 536 18.4 DDM Drivers���������������������������������������������������������������������������������� 538 18.5 Manufacturing Versus Prototyping ������������������������������������������������ 540 18.6 Cost Estimation������������������������������������������������������������������������������ 542 18.6.1 Cost Model������������������������������������������������������������������������ 542 18.6.2 Build Time Model������������������������������������������������������������ 544 18.6.3 Laser Scanning Vat Photopolymerization Example���������� 547 18.7 Life-Cycle Costing�������������������������������������������������������������������������� 548 18.8 Future of Direct Digital Manufacturing������������������������������������������ 550 18.9 Questions���������������������������������������������������������������������������������������� 551 References�������������������������������������������������������������������������������������������������� 553 19 Design for Additive Manufacturing�������������������������������������������������������� 555 19.1 Introduction������������������������������������������������������������������������������������ 555 19.2 Design for Manufacturing and Assembly �������������������������������������� 556 19.3 Core DFAM Concepts and Objectives�������������������������������������������� 559 19.3.1 Opportunistic vs. Restrictive DFAM�������������������������������� 559 19.3.2 AM Unique Capabilities �������������������������������������������������� 560 19.3.3 Shape Complexity������������������������������������������������������������ 560 19.3.4 Hierarchical Complexity�������������������������������������������������� 561 19.3.5 Functional Complexity������������������������������������������������������ 563 19.3.6 Material Complexity �������������������������������������������������������� 565
19.4 Design Opportunities���������������������������������������������������������������������� 567 19.4.1 Part Consolidation Overview�������������������������������������������� 567 19.4.2 Design for Function���������������������������������������������������������� 569 19.4.3 Part Consolidation Consequences������������������������������������ 571 19.4.4 Customized Geometry������������������������������������������������������ 572 19.4.5 Hierarchical Structures����������������������������������������������������� 572 19.4.6 Multifunctional Designs��������������������������������������������������� 574 19.4.7 Elimination of Conventional DFM Constraints���������������� 575 19.4.8 Industrial Design Applications������������������������������������������ 576 19.4.9 Role of Design Standards������������������������������������������������� 578 19.5 Design for Four-Dimensional (4D) Printing���������������������������������� 578 19.5.1 Definition of 4D Printing�������������������������������������������������� 579 19.5.2 Shape-Shifting Mechanisms and Stimuli�������������������������� 580 19.5.3 Shape-Shifting Types and Dimensions ���������������������������� 581 19.6 Computer-Aided Design Tools for AM������������������������������������������ 583 19.6.1 Challenges for CAD���������������������������������������������������������� 583 19.6.2 Solid Modeling CAD Technologies���������������������������������� 584 19.6.3 Commercial CAD Capabilities ���������������������������������������� 586 19.6.4 Prototypical DFAM System���������������������������������������������� 587 19.7 Design Space Exploration�������������������������������������������������������������� 591 19.7.1 Design of Experiments������������������������������������������������������ 591 19.7.2 Design Exploration Software�������������������������������������������� 593 19.8 Synthesis Methods�������������������������������������������������������������������������� 594 19.8.1 Theoretically Optimal Lightweight Structures ���������������� 594 19.8.2 Optimization Methods������������������������������������������������������ 595 19.8.3 Topology Optimization ���������������������������������������������������� 596 19.9 Summary ���������������������������������������������������������������������������������������� 604 19.10 Questions���������������������������������������������������������������������������������������� 604 References�������������������������������������������������������������������������������������������������� 605 20 Rapid Tooling ������������������������������������������������������������������������������������������ 609 20.1 Introduction������������������������������������������������������������������������������������ 609 20.2 Direct AM Production of Injection Molding Inserts���������������������� 611 20.3 EDM Electrodes������������������������������������������������������������������������������ 616 20.4 Investment Casting�������������������������������������������������������������������������� 616 20.5 Other Systems �������������������������������������������������������������������������������� 618 20.5.1 Vacuum Forming Tools ���������������������������������������������������� 618 20.5.2 Paper Pulp Molding Tools������������������������������������������������ 618 20.5.3 Formwork for Composite Manufacture���������������������������� 619 20.5.4 Assembly Tools and Metrology Registration Rigs ���������� 620 20.6 Questions���������������������������������������������������������������������������������������� 620 References�������������������������������������������������������������������������������������������������� 621 21 Industrial Drivers for AM Adoption������������������������������������������������������ 623 21.1 Introduction������������������������������������������������������������������������������������ 623 21.2 Historical Developments���������������������������������������������������������������� 624
21.2.1 Value of Physical Models������������������������������������������������� 624 21.2.2 Functional Testing������������������������������������������������������������ 625 21.2.3 Rapid Tooling�������������������������������������������������������������������� 626 21.3 The Use of AM to Support Medical Applications�������������������������� 627 21.3.1 Surgical and Diagnostic Aids�������������������������������������������� 628 21.3.2 Prosthetics and Implants �������������������������������������������������� 630 21.3.3 Tissue Engineering and Organ Printing���������������������������� 632 21.4 Software Tools and Surgical Guides for Medical Applications������������������������������������������������������������������������������������ 633 21.5 Limitations of AM for Medical Applications���������������������������������� 634 21.5.1 Speed�������������������������������������������������������������������������������� 635 21.5.2 Cost ���������������������������������������������������������������������������������� 636 21.5.3 Accuracy �������������������������������������������������������������������������� 636 21.5.4 Materials �������������������������������������������������������������������������� 637 21.5.5 Ease of Use ���������������������������������������������������������������������� 637 21.6 Further Development of Medical AM Applications ���������������������� 637 21.6.1 Approvals�������������������������������������������������������������������������� 638 21.6.2 Insurance �������������������������������������������������������������������������� 638 21.6.3 Engineering Training�������������������������������������������������������� 639 21.6.4 Location of the Technology���������������������������������������������� 639 21.6.5 Service Bureaus���������������������������������������������������������������� 639 21.7 Aerospace Applications������������������������������������������������������������������ 640 21.7.1 Characteristics Favoring AM�������������������������������������������� 640 21.7.2 Production Manufacture���������������������������������������������������� 641 21.8 Automotive Applications���������������������������������������������������������������� 644 21.9 Questions���������������������������������������������������������������������������������������� 645 References�������������������������������������������������������������������������������������������������� 646
22 Business and Societal Implications of AM �������������������������������������������� 649 22.1 Introduction������������������������������������������������������������������������������������ 649 22.2 What Could Be New? �������������������������������������������������������������������� 651 22.2.1 New Types of Products ���������������������������������������������������� 651 22.2.2 New Types of Organizations �������������������������������������������� 653 22.2.3 New Types of Employment���������������������������������������������� 656 22.3 Digiproneurship������������������������������������������������������������������������������ 657 22.4 Summary ���������������������������������������������������������������������������������������� 660 22.5 Questions���������������������������������������������������������������������������������������� 661 References�������������������������������������������������������������������������������������������������� 661 Index������������������������������������������������������������������������������������������������������������������ 663
Introduction and Basic Principles
Abstract The technology described in this book was originally referred to as Rapid Prototyping. The term Rapid Prototyping (or RP) is used to describe a process for rapidly creating a system or part representation before final release or commercialization. The emphasis is on creating something quickly for use as a prototype or basis model from which further models and eventually the final product will be derived. In product development, the term Rapid Prototyping describes technologies which create physical prototypes. This text is about technologies which can directly produce objects from digital data. These technologies were first developed for prototyping but are now used for many more purposes.
1.1 What Is Additive Manufacturing? Additive Manufacturing is the formalized term for what used to be called Rapid Prototyping and what is popularly called 3D Printing. The term Rapid Prototyping (or RP) is used in a variety of industries to describe a process for rapidly creating a system or part representation before final release or commercialization. In other words, the emphasis is on creating something quickly, and that the output is a prototype or basis model from which further models and eventually the final product will be derived. Management consultants and software engineers both also use the term Rapid Prototyping to describe a process of developing business and software solutions in a piecewise fashion that allows clients and other stakeholders to test ideas and provide feedback during the development process. In a product development context, the term Rapid Prototyping was used widely to describe technologies which created physical prototypes directly from digital model data. This text is about these latter technologies, first developed for prototyping but now used for many more purposes. Users of RP technology have come to realize that this term is inadequate and in particular does not effectively describe more recent applications of the technology. © Springer Nature Switzerland AG 2021 I. Gibson et al., Additive Manufacturing Technologies, https://doi.org/10.1007/978-3-030-56127-7_1
1 Introduction and Basic Principles
Improvements in the quality of the output from these machines have meant that there is often a much closer link to the final product. Many parts are in fact now directly manufactured in these machines, so it is not possible for us to label them as “prototypes.” The term Rapid Prototyping also overlooks the basic principle of these technologies in that they all fabricate parts using an additive approach. A Technical Committee within ASTM International agreed that new terminology should be adopted. As a result, ASTM consensus standards now use the term Additive Manufacturing  as do most standards bodies worldwide. Referred to in short as AM, the basic principle of this technology is that a model, initially generated using a three-dimensional Computer Aided Design (3D CAD) system, can be fabricated directly without the need for process planning. Although this is not in reality as simple as it first sounds, AM technology significantly simplifies the process of producing complex 3D objects directly from CAD data. Other manufacturing processes require a careful and detailed analysis of the part geometry to determine things like the order in which different features can be fabricated, what tools and processes must be used, and what additional fixtures may be required to complete the part. In contrast, AM needs only some basic dimensional details and a small amount of understanding as to how the AM machine works and the materials that are used to build the part. The key to how AM works is that parts are made by adding material in layers; each layer is a thin cross-section of the part derived from the original CAD data. Obviously in the physical world, each layer must have a finite thickness to it, and so the resulting part will be an approximation of the original data, as illustrated by Fig. 1.1. The thinner each layer is, the closer the final part will be to the original. All commercialized AM machines to date use a layer-based approach, and the major ways that they differ are in the materials that can be used, how the layers are created,
Fig. 1.1 CAD image of a teacup with further images showing the effects of building using different layer thicknesses
1.3 The Generic AM Process
and how the layers are bonded to each other. Such differences will determine factors like the accuracy of the final part plus its material properties and mechanical properties. They will also determine factors like how quickly the part can be made, how much post-processing is required, the size of the AM machine used, and the overall cost of the machine and process. This chapter will introduce the basic concepts of Additive Manufacturing and describe a generic AM process from design to application. It will go on to discuss the implications of AM on design and manufacturing and attempt to help in understanding how it has changed the entire product development process. Since AM is an increasingly important tool for product development, the chapter ends with a discussion of some related tools in the product development process.
1.2 What Are AM Parts Used For? Throughout this book you will find a wide variety of applications for AM. You will also realize that the number of applications is increasing as the processes develop and improve. Initially, AM was used specifically to create visualization models for products as they were being developed. It is widely known that models can be much more helpful than drawings or renderings in fully understanding the intent of the designer when presenting the conceptual design. While drawings are quicker and easier to create, models are nearly always required in the end to fully validate the design. Following this initial purpose of simple model making, AM technology has developed over time as materials, accuracy, and the overall quality of the output improved. Models were quickly employed to supply information about what is known as the “3 Fs” of Form, Fit, and Function. The initial models were used to help fully appreciate the shape and general purpose of a design (Form). Improved accuracy in the process meant that components were capable of being built to the tolerances required for assembly purposes (Fit). Improved material properties meant that parts could be properly handled so that they could be assessed according to how they would eventually work (Function). To say that AM technology is only useful for making models, though, would be inaccurate and undervaluing the technology. AM, when used in conjunction with other technologies to form process chains, can be used to significantly shorten product development times and costs. More recently, some of these technologies have been developed to the extent that the output is suitable for end use. This explains why the terminology has essentially evolved from Rapid Prototyping to Additive Manufacturing.
1.3 The Generic AM Process AM involves a number of steps that move from the virtual CAD description to the physical resultant part. Different products will involve AM in different ways and to different degrees. Small, relatively simple products may only make use of AM for
1 Introduction and Basic Principles
visualization models, while larger, more complex products with greater engineering content may involve AM during numerous stages and iterations throughout the development process. Furthermore, early stages of the product development process may only require rough parts, with AM being used because of the speed at which they can be fabricated. At later stages of the process, parts may require careful cleaning and post-processing (including sanding, surface preparation, and painting) before they are used, with AM being useful here because of the complexity of form that can be created without having to consider tooling. Later on, we will investigate thoroughly the different stages of the AM process, but to summarize, most AM processes involve, to some degree at least, the following eight steps (as illustrated in Fig. 1.2).
1.3.1 Step 1: CAD All AM parts must start from a software model that fully describes the external geometry. This can involve the use of almost any professional CAD solid modeling software, but the output must be a 3D solid or surface representation. Reverse engineering equipment (e.g., laser and optical scanning) can also be used to create this representation.
1 CAD 2 STL convert 3 File transfer to machine 4 Machine setup 5 Build 6 Remove 7 Post-process 8 Application
Fig. 1.2 Generic process of CAD to part, showing all eight stages
1.3 The Generic AM Process
1.3.2 Step 2: Conversion to STL Nearly every AM machine accepts the STL file format, which has become a de facto standard, and nowadays nearly every CAD system can output such a file format. This file describes the external closed surfaces of the original CAD model and forms the basis for calculation of the slices.
1.3.3 S tep 3: Transfer to AM Machine and STL File Manipulation The STL file describing the part must be transferred to the AM machine. Here, there may be some general manipulation of the file so that it is the correct size, position, and orientation for building.
1.3.4 Step 4: Machine Setup The AM machine must be properly set up prior to the build process. Such settings would relate to the build parameters like the material constraints, energy source, layer thickness, timings, etc.
1.3.5 Step 5: Build Building the part is mainly an automated process, and the machine can largely carry on without supervision. Only superficial monitoring of the machine needs to take place at this time to ensure no errors have taken place like running out of material, power or software glitches, etc.
1.3.6 Step 6: Removal Once the AM machine has completed the build, the parts must be removed. This may require interaction with the machine, which may have safety interlocks to ensure, for example, that the operating temperatures are sufficiently low or that there are no actively moving parts.
1 Introduction and Basic Principles
1.3.7 Step 7: Post-Processing Once removed from the machine, parts may require an amount of additional cleaning up before they are ready for use. Parts may be weak at this stage, or they may have supporting features that must be removed. They may require priming and painting to give an acceptable surface texture and finish. This step may also involve heat treatment. Post-processing may be costly, laborious, and lengthy if the finishing requirements are very demanding.
1.3.8 Step 8: Application Parts are now ready for use. This may require them to be assembled together with other mechanical or electronic components to form a final model or product. While the numerous stages in the AM process have now been discussed, it is important to realize that other steps may be needed for certain machines and processes. For example, certain machine setup software and AM machines may be compatible with native CAD information, and thus the STL file may be skipped. In addition, many AM machines require careful maintenance. Many AM machines use fragile laser or printer technology that must be carefully monitored and that should preferably not be used in a dirty or noisy environment. While machines are generally designed to operate unattended, it is important to include regular checks in the maintenance schedule, and that different technologies and/or applications require different levels of maintenance. There is an increasing use of materials and process standards for AM, and the ASTM F42 Technical Committee on Additive Manufacturing Technologies is working to add more . Maintenance standards may be more strict for certain applications than for others. In addition, many machine vendors recommend and provide test patterns and maintenance guidance that can be used periodically to confirm that machines are operating within acceptable limits. In addition to the machinery, materials may also require careful handling. The raw materials used in some AM processes have limited shelf life and may also be required to be kept in conditions that prevent them from unwanted chemical reactions. Exposure to moisture, excess light, and other contaminants should also be avoided. Most processes use materials that can be reused for more than one build. However, it may be that reuse could degrade the properties if performed many times over, and therefore a procedure for maintaining consistent material quality through recycling should also be observed.
1.4 Why Use the Term Additive Manufacturing? By now, you should realize that the technology we are referring to is primarily the use of additive processes, combining materials layer-by-layer. The term Additive Manufacturing, or AM, seems to describe this quite well, but there are many other
1.4 Why Use the Term Additive Manufacturing?
terms which are in use. This section discusses other terms that have been used to describe this technology as a way of explaining the overall purpose and benefits of the technology for product development.
1.4.1 Automated Fabrication (Autofab) This term was popularized by Marshall Burns in his book of the same name, which was one of the first texts to cover AM technology in the early 1990s . The emphasis here is on the use of automation to manufacture products, thus implying the simplification or removal of manual tasks from the process. Computers and microcontrollers are used to control the actuators and to monitor the system variables. This term can also be used to describe other forms of Computer Numerical Controlled (CNC) machining centers since there is no direct reference as to how parts are built or the number of stages it would take to build them, although Burns does primarily focus on the technologies also covered by this book. Some key technologies are however omitted since they arose after the book was written.
1.4.2 Freeform Fabrication or Solid Freeform Fabrication The emphasis here is in the capability of the processes to fabricate complex geometric shapes. Sometimes the advantage of these technologies is described in terms of providing “complexity for free,” implying that it doesn’t particularly matter what the shape of the input object actually is. A simple cube or cylinder would take almost as much time and effort to fabricate within the machine as a complex anatomical structure with the same enclosing volume. The reference to “freeform” relates to the independence of form from the manufacturing process. This is very different from most conventional manufacturing processes that become much more involved as the geometric complexity increases.
1.4.3 Additive Manufacturing or Layer-Based Manufacturing These descriptions relate to the way the processes fabricate parts by adding material in layers. This is in contrast to machining technology that removes or subtracts material from a block of raw material. It should be noted that some of the processes are not purely additive, in that they may add material at one point but also use subtractive processes at some stage as well. Currently, every commercial process works in a layer-wise fashion. However, there is nothing to suggest that this is an essential approach to use and that future systems may add material in other ways and yet still come under a broad classification that is appropriate to this text. A slight variation
1 Introduction and Basic Principles
on this, Additive Fabrication, is a term that was popularized by Terry Wohlers, a well-known industry consultant in this field and who compiles a widely regarded annual industry report on the state of this industry . However, the term “manufacturing” tends to be the more general term, and, in fact, “Additive Manufacturing” is now the international standard term used to refer to this class of manufacturing processes . Originally approved in 2009 by the ASTM F42 Committee, Additive Manufacturing was adopted as the official name for the technology, along with the names of the seven identified classes of AM processes.
1.4.4 Rapid Prototyping Rapid Prototyping was termed because of the process this technology was designed to enhance or replace. Manufacturers and product developers used to find prototyping a complex, tedious, and expensive process that often impeded the developmental and creative phases during the introduction of a new product. RP was found to significantly speed up this process, and thus the term was adopted. However, users and developers of this technology now realize that AM technology can be used for much more than just prototyping. Significant improvements in accuracy and material properties have seen this technology catapulted into testing, tooling, manufacturing, and other realms that are outside the “prototyping” definition.
1.4.5 Stereolithography or 3D Printing These two terms were initially used to describe specific machines. Stereolithography (SL) was termed by the US company 3D Systems [5, 6], and 3D Printing (3DP) was widely used by researchers at MIT  who invented an inkjet printing-based technology. Both terms allude to the use of 2D processes (lithography and printing) and extending them into the third dimension. Since most people are very familiar with printing technology, the idea of printing a physical three-dimensional object should make sense. Many consider that eventually the term 3D Printing will become the most commonly used wording to describe AM technologies. Recent media interest in the technology has proven this to be true, and the general public is much more likely to know the term 3D Printing than any other term mentioned in this book. We use Additive Manufacturing or its abbreviation AM throughout this book as the generic term for the suite of technologies covered by this book as this is the terminology used by experts and standards bodies. It should be noted that, in the literature, most of the terms introduced above are interchangeable; but different terminology may emphasize the approach used in a particular instance. Thus, both in this book and while searching for or reading other literature, the reader must consider the context to best understand what each of these terms means.
1.5 The Benefits of AM
1.5 The Benefits of AM Many people have described AM as revolutionizing product development and manufacturing. Some have even gone on to say that manufacturing, as we know it today, may not exist if we follow AM to its ultimate conclusion and that we are experiencing a new industrial revolution. AM is now frequently referred to as one of a series of disruptive technologies that are changing the way we design products and set up new businesses. We might, therefore, like to ask “why is this the case?” What is it about AM that enthuses and inspires some to make these kinds of statements? First, let’s consider the “rapid” character of this technology. The speed advantage is not just in terms of the time it takes to build parts. The speeding up of the whole product development process relies much on the fact that we are using computers throughout. Since 3D CAD is being used as the starting point and the transfer to AM is relatively seamless, there is much less concern over data conversion or interpretation of the design intent. Just as 3D CAD is becoming What You See Is What You Get (WYSIWYG), so it is the same with AM, and we might just as easily say that What you See Is What You Build (WYSIWYB). The seamlessness can also be seen in terms of the reduction in process steps. Regardless of the complexity of parts to be built, building within an AM machine is generally performed in a single step. Most other manufacturing processes would require multiple and iterative stages to be carried out. As you include more features in a design, the number of these stages may increase dramatically. Even a relatively simple change in the design may result in a significant increase in the time required to build using conventional methods. The amount of time to fabricate models using AM, however, is relatively insensitive to simple design changes that may be implemented during this formative stage of product development. Similarly, the number of processes and resources required can be significantly reduced when using AM. If a skilled craftsman was requested to build a prototype according to a set of CAD drawings, he may find that he must manufacture the part in a number of stages. This may be because he must employ a variety of construction methods, ranging from hand carving, through molding and forming techniques, to CNC machining. Hand carving and similar operations are tedious, difficult, and prone to error. Molding technology can be messy and obviously requires the building of one or more molds. CNC machining requires careful planning and a sequential approach that may also require construction of fixtures before the part itself can be made. All this of course presupposes that these technologies are within the repertoire of the craftsman and readily available. AM can be used to remove or at least simplify many of these multistage processes. With the addition of some supporting technologies like silicone–rubber molding, drills, polishers, grinders, etc., it can be possible to manufacture a vast range of different parts with different characteristics. Workshops which adopt AM technology can be much cleaner, more streamlined, and more versatile than before.
1 Introduction and Basic Principles
1.6 Distinction Between AM and Conventional Manufacturing Processes As mentioned in the discussion on Automated Fabrication, AM shares some of its DNA with conventional manufacturing technologies like Computer Numerical Controlled (CNC) machining. CNC technologies in general are computer-based manufacturing technologies. Conventional technologies are often divided into subtractive, casting, and forming technologies. All can use CNC controllers to increase the accuracy and better control the process. In subtractive manufacturing, such as CNC machining, materials are removed by contact with cutting tools, and therefore chips are produced. In forming the forming tool changes the shape of sheet or blocks of material by exerting high forces, and chips are not generated. In casting, molten material is directed into a mold. CNC machining is capable of making complex parts directly from CAD data but in a subtractive rather than additive way. CNC machining requires a block of material that must be at least as big as the part that is to be made. In AM powders, filaments, liquids, or other feedstocks are added together to create a part that is larger than the feedstock in one or more dimensions. This section discusses a range of topics where comparisons between CNC machining and AM are made. The purpose is not to influence choice of one technology over another but rather to establish how they may be implemented for different stages in the product development process or for different types of product.
1.6.1 Material AM technology was originally developed around polymeric materials, waxes, and paper laminates. Subsequently, there has been introduction of composites, metals, and ceramics. CNC machining can be used for soft materials, like medium-density fiberboard (MDF), machineable foams, machineable waxes, and even some polymers. However, use of CNC to shape softer materials is typically focused on preparing these parts for use in a multistage process like casting. When using CNC machining to make final products, it works particularly well for hard, relatively brittle materials like steels and other metal alloys to produce high accuracy parts with well-defined properties. Some AM parts, in contrast, may have voids or anisotropy that are a function of part orientation, process parameters, or how the design was input to the machine, whereas CNC parts will normally be more homogeneous and predictable in quality.
1.6.2 Speed High-speed CNC machining can generally remove material much faster than AM machines can add a similar volume of material. However, this is only part of the picture, as AM technology can be used to produce a part in a single stage. CNC
1.6 Distinction Between AM and Conventional Manufacturing Processes
machines require considerable setup and process planning, particularly as parts become more complex in their geometry. Speed must therefore be considered in terms of the whole process rather than just the physical interaction with the part material. CNC is likely to be a multistage manufacturing process, requiring repositioning or relocation of parts within one machine or use of more than one machine. To make a part in an AM machine, it may only take a few hours; and in fact multiple parts are often batched together inside a single AM build. Finishing may take a few days if the requirement is for high quality. Using CNC machining, even 5-axis highspeed machining, this same process may take weeks for high complexity parts, with considerably more uncertainty over the completion time. This is due to the complex planning involved and custom jigs and fixtures needed to make the part the first time. For the second and subsequent parts, however, CNC machining may be faster than AM.
1.6.3 Complexity As mentioned above, the higher the geometric complexity, the greater the advantage AM has over CNC. If CNC is being used to create a part directly in a single piece, then there may be some geometric features that cannot be fabricated. Since a machining tool must be carried in a spindle, there may be certain accessibility constraints or clashes preventing the tool from being located on the machining surface of a part. AM processes are not constrained in the same way, and undercuts and internal features can be easily built without specific process planning. Certain parts cannot be fabricated by CNC unless they are broken up into components and reassembled at a later stage. Consider, for example, the possibility of machining a ship inside a bottle. How would you machine the ship while it is still inside the bottle? Most likely you would machine both elements separately and work out a way to combine them together as an assembly and/or joining process. With AM you can build the ship and the bottle all at once. An expert in machining must therefore analyze each part prior to it being built to ensure that it indeed can be built and to determine what methods need to be used. While it is still possible that some parts cannot be built with AM, the likelihood is much lower, and there are generally ways in which this may be overcome without too much difficulty.
1.6.4 Accuracy AM machines generally operate with a resolution of a few tens of microns. It is common for AM machines to also have different resolution along different orthogonal axes. Typically, the vertical build axis corresponds to layer thickness, and this would be of a lower resolution compared with the resolution of the two axes in the build plane. Accuracy in the build plane is determined by the positioning of the
1 Introduction and Basic Principles
build mechanism, which will normally involve gearboxes and motors of some kind. This mechanism may also determine the minimum feature size as well. For example, stereolithography uses a laser as part of the build mechanism that will normally be positioned using galvanometric mirror drives. The resolution of the galvanometers would determine the overall dimensions of parts built, while the diameter of the laser beam would determine the minimum wall thickness. The accuracy of CNC machines on the other hand is mainly determined by a similar positioning resolution along all three orthogonal axes and by the diameter of the rotary cutting tools. There are factors that are defined by the tool geometry, like the radius of internal corners, but wall thickness can be thinner than the tool diameter since it is a subtractive process. In both cases very fine detail will also be a function of the desired geometry and properties of the build material.
1.6.5 Geometry AM machines essentially break up a complex, 3D problem into a series of simple 2D cross-sections with a nominal thickness. In this way, the connection of surfaces in 3D is removed, and continuity is determined by how close the proximity of one cross-section is with an adjacent one. Since this cannot be easily done in CNC, machining of surfaces must normally be generated in 3D space. With simple geometries, like cylinders, cuboids, cones, etc., this is a relatively easy process defined by joining points along a path, these points being quite far apart and the tool orientation being fixed. In cases of freeform surfaces, these points can become very close together with many changes in orientation. Such geometry can become extremely difficult to produce with CNC, even with 5-axis interpolated control or greater. Undercuts, enclosures, sharp internal corners, and other features can all fail if these features are beyond a certain limit. Consider, for example, the features represented in the part in Fig. 1.3. Many of them would be very difficult to machine without manipulation of the part at various stages.
1.6.6 Programming Determining the program sequence for a CNC machine can be very involved, including tool selection, machine speed settings, approach position and angle, etc. Many AM machines also have options that must be selected, but the range, complexity, and implications surrounding their choice are minimized when using pre- configured process parameter combinations. The worst that is likely to happen in most AM machines is that the part will not be built very well if the programming and process parameter selection is not done properly. Incorrect programming of a CNC machine could result in severe damage to the machine and may even be a human safety risk.
1.7 Example AM Parts
The cavity here may be too deep to machine
The undercut here cannot be performed without more than 3 axis machining
Curved features cannot be machined without a form mill cutter Base cannot be machined without holding the cup in a custom fixture
Fig. 1.3 Features that represent problems using CNC machining
1.7 Example AM Parts Figure 1.4 shows a montage of parts fabricated using some of the common AM processes. Part a. was fabricated using a stereolithography machine and depicts a simplified fuselage for an unmanned aerial vehicle where the skin is reinforced with a conformal lattice structure (see Chap. 4 for more information about the process). A more complete description of this part is included in the Design for Additive Manufacturing chapter. Parts b. and c. were fabricated using material jetting (Chap. 7). Part b. demonstrates the capability of depositing multiple materials simultaneously, where one set of nozzles deposited the clear material, while another set deposited the black material for the lines and the Objet name. Part c. is a section of chain. Both parts b. and c. have working revolute joints that were fabricated using clearances for the joints and dissolvable support structures. Part d. is a metal part that was fabricated in a metal Powder Bed Fusion (PBF) machine using an electron beam as its energy source (Chap. 5). The part is a model of a facial implant. Part e. was fabricated in an Mcor Technologies Sheet Lamination machine that has inkjet printing capability for the multiple colors (Chap. 9). Parts f. and g. were fabricated using Material Extrusion (MEX) (Chap. 6). Part f. is a ratchet mechanism that was fabricated in a single build in an industrial machine. Again, the working mechanism is achieved through proper joint designs and dissolvable support structures. Part g. was fabricated in a low-cost, MEX machine (that one of the authors has at home). Parts h. and i. were fabricated using polymer PBF. Part h. is the well-known “brain gear” model of a three-dimensional gear train. When one gear is rotated, all other gears rotate as well. Since parts fabricated in polymer PBF do not need supports, working revolute and gear joints can be created by managing clearances and remov-
1 Introduction and Basic Principles
Fig. 1.4 Montage of AM parts
ing the loose powder from the joint regions. Part i. is another conformal lattice structure showing the shape complexity capability of AM technologies.
1.8 Other Related Technologies The most common input method for AM technology is to accept a file converted into the STL file format originally built within a conventional 3D CAD system. There are, however, other ways in which the STL files can be generated and other technologies that can be used in conjunction with AM technology. This section will describe a few of these.
1.8.1 Reverse Engineering Technology More and more models are being built from data generated using reverse engineering (RE) 3D imaging equipment and software. In this context, RE is the process of capturing geometric data from another object. These data are usually initially available in what is termed “point cloud” form, meaning an unconnected set of points representing the object surfaces. These points need to be connected together using RE software like Geomagic , which may also be used to combine point clouds from different scans and to perform other functions like hole-filling and smoothing.
1.8 Other Related Technologies
In many cases, the data will not be entirely complete. Samples may, for example, need to be placed in a holding fixture, and thus the surfaces adjacent to this fixture may not be scanned. In addition, some surfaces may obscure others, like with deep crevices and internal features, so that the representation may not turn out exactly how the object is in reality. Recently there have been huge improvements in scanning technology. An adapted smartphone using its in-built camera can now produce a high-quality 3D scan for just a few hundred dollars that even just a few years ago would have required an expensive laser scanning or stereoscopic camera system costing $100,000 or more. Engineered objects would normally be scanned using laser scanning or touch probe technology. Objects that have complex internal features or anatomical models may make use of Computerized Tomography (CT), which was initially developed for medical imaging but is also available for scanning industrially produced objects. This technique essentially works in a similar way to AM, by scanning layer-by-layer and using software to join these layers and identify the surface boundaries. Boundaries from adjacent layers are then connected together to form surfaces. The advantage of CT technology is that internal features can also be generated. High-energy X-rays are used in industrial technology to create high-resolution images of around 1 μm. Another approach that can help digitize objects is the Capture Geometry Inside  technology that also works very much like a reverse of AM technology, where 2D imaging is used to capture cross-sections of a part as it is machined away layer-by-layer. Obviously this is a destructive approach to geometry capture so it cannot be used for every type of product. AM can be used to reproduce the articles that were scanned, which essentially would form a kind of 3D facsimile (3D Fax) process. More likely, however, the data will be modified and/or combined with other data to form complex, freeform artifacts that are taking advantage of the “complexity for free” feature of the technology. An example may be where individual patient data are combined with an engineering design to form a customized medical implant. This is something that will be discussed in more detail later in this book.
1.8.2 Computer-Aided Engineering/Technologies (CAX) CAX is the use of computer technologies to aid in the design, analysis, and manufacture of products. Computer-Aided Engineering (CAE) is the wide usage of computer software to help engineers analyze their tasks using simulation. Other major CAX sub-categories include Computer-Aided Design (CAD) and Computer-Aided Manufacturing (CAM).
1 Introduction and Basic Principles
126.96.36.199 Computer-Aided Design (CAD) CAD is the use of a computer to aid in the creation, design, modification, analysis, and optimization of a component. CAD software helps increase the efficiency and quality of the design process and enhances communication through documentation by generating organized databases. One of the features of most CAD software is an ability to create electronic output files for printing, machining, or other manufacturing operations. CT images can be converted to CAD files using various software packages, and subsequent modifications can be performed. For instance, to fill the worn part of a bone in the spinal column, CT scan images can be converted to 3D images, and the worn part can be modified and filled. Then in the next step, the file can be saved as an STL file and sent directly to an AM machine for printing. 3D CAD is an extremely valuable resource for product design and development. One major benefit to using software-based design is the ability to implement changes easily and cheaply. If we are able to keep the design primarily in a software format for a larger proportion of the product development cycle, we can ensure that any design changes are performed virtually on the software description rather than physically on the product itself. The more we know about how the product is going to perform before it is built, the more effective that product is going to be. This is also the most cost-effective way to deal with product development. If problems are only noticed after parts are physically manufactured, this can be very costly. 3D CAD can make use of AM to help visualize and perform basic tests on candidate designs prior to full-scale commitment to manufacturing. However, the more complex and performance-related the design, the less likely we are to gain sufficient insight using these methods. 3D CAD is commonly linked to other software packages, often using techniques like the Finite Element Method (FEM) to calculate the mechanical response of a design to certain stimuli, collectively known as Computer-Aided Engineering (CAE). Forces, dynamics, stresses, flow, heat, and other responses can be predicted to determine how well a design will perform under certain conditions. While such software cannot easily predict the exact behavior of a part, for analysis of critical parts, a combination of CAE, backed up with AM-based experimental analysis, may be a useful solution. Further, with the advent of Direct Digital Manufacture, where AM can be used to directly produce final products, there is an increasing need for CAE tools to evaluate how these parts would perform prior to AM so that we can build these products right the first time.
1.8.3 Haptic-Based CAD 3D CAD systems are generally built on the principle that models are constructed from basic geometric shapes that are then combined in different ways to make more complex forms. This works very well for the engineered products we are familiar with but may not be so effective for more unusual designs. Many consumer products
1.8 Other Related Technologies
are developed from ideas generated by artists and designers rather than engineers. We also note that AM has provided a mechanism for greater freedom of expression. AM is in fact now becoming a popular tool for artists and sculptors, like, for example, Bathsheba Grossman  who takes advantage of the geometric freedom to create visually exciting sculptures (including the one shown on the cover of this book). One problem we face today is that some computer-based design tools constrain or restrict creative processes and there is scope for a CAD system that provides greater freedom. Haptic-based CAD modeling systems like the experimental system shown in Fig. 1.5  work in a similar way to commercially available freeform  modeling systems to provide a design environment that is more intuitive than standard CAD systems. In this image a robotic haptic feedback device called the Phantom provides force feedback relating to the virtual modeling environment. An object can be seen on screen but also felt in 3D space using the Phantom. The modeling environment includes what is known as Virtual Clay that deforms under force applied using the haptic cursor. This provides a mechanism for direct interaction with the modeling material, much like how a sculptor interacts with actual clay. The results using this system are generally much more organic and freeform than the surfaces that can be incorporated into product designs by using traditional engineering CAD tools. As consumers become more demanding and discerning, we can see that CAD tools for non-engineers like designers, sculptors, and even members of the general public are likely to become much more commonplace.
Fig. 1.5 Freeform modeling system
1 Introduction and Basic Principles
188.8.131.52 Computer-Aided Manufacturing (CAM) CAM is the use of a computer to control machine tools in order to fabricate a component. The initial purpose of CAM was increasing the speed of manufacturing processes and simultaneously increasing the accuracy, consistency, and precision of manufacturing combined with a reduction of lead time and energy. The first CAM systems used an individual programmer to create and develop a solution by code writing and manually changing controller options. After significant trial and error, a successful “recipe” would be developed that could be used repeatedly to create identical components. Initial systems were numerically controlled (NC), and the codes were fed into a machine using punch cards. The programs in the NC machine could not be stored and had less flexibility, accuracy, and productivity and also required an expert programmer. The next generation was Computer Numerical Controlled (CNC), where a computer directly controlled the motion of the tool. The programs were fed into the machine directly from computers. In CNC, modification of the programs were greatly simplified. Today, the connection between CAD and CAM is simple and efficient in many software tools. 184.108.40.206 Computer-Aided Engineering (CAE) CAE is the use of a computer to simulate the effects of various physics applied to a component or system. Today’s multi-physics simulation tools are powerful complements to AM. Topology optimization and generative design are commonly used by designers to guide them to a part shape which is the lowest weight component capable of achieving a certain task. AM process simulation tools are a relatively new set of CAE tools, introduced into the market over the past few years. These AM process simulation tools can predict distortion, microstructure, porosity, and other characteristics of an AM part prior to its creation. By simulating the effects of an AM process on a specific geometry, build failures can be reduced, and shape changes that occur in the part can be compensated for prior to production, so that the part can be produced to a higher tolerance and with a higher probability of success .
1.9 About This Book There have been a number of texts describing additive manufacturing processes, either as dedicated books or as sections in other books. Prior to the first edition of this book, however, there were no texts dedicated to presenting this technology in a comprehensive way within a university setting. Universities are incorporating additive manufacturing into various curricula. This has varied from segments of single modules to complete postgraduate courses. This text is aimed at supporting these curricula with a comprehensive coverage of as many aspects of this technology as possible. The authors of this text have all been involved in setting up programs in
their home universities and have written this book because they feel that there were no books that covered the required material in sufficient breadth and depth. Furthermore, with the increasing interest in Additive Manufacturing and 3D Printing, we believe that this text can also provide a comprehensive understanding of the technologies involved. Despite increased popularity, it is clear that there is a significant lack of basic understanding by many of the breadth that AM has to offer. Early chapters in this book discuss general aspects of AM, followed by chapters which focus on specific AM technologies. The final chapters focus more on generic processes and applications. It is anticipated that the reader will be familiar with 3D solid modeling CAD technology and have at least a small amount of knowledge about product design, development, and manufacturing. The majority of readers would be expected to have an engineering or design background, more specifically product design, or mechanical, materials, or manufacturing engineering. Since AM technology also involves significant electronic and information technology components, readers with a background in computer applications and mechatronics may also find this text beneficial. This third edition has been comprehensively overhauled in an attempt to bring it up to date with the extremely fast-moving landscape of AM. All references have been checked and updated, with many more web-based sources. All images have been checked, with many diagrams redrawn for greater clarity. Replacement photographs show more recent technologies where appropriate. There is much more detail regarding processes and, in particular, on materials. A new chapter on AM materials helps readers understand how new materials are being developed. In particular, there is increasing focus on high performance materials, including ceramics and multi-phase, multi-material structures. We have included as many of these new concepts as we could to show how this exciting domain continues to develop. Finally, we recognize that many educators are including this book as a core text. To help, we have revamped the end of chapter questions as part of a larger process aimed at helping with curriculum development.
1.10 Questions 1. Find three other definitions for Rapid Prototyping other than that of Additive Manufacturing as covered by this book. 2. From the web, find different examples of applications of AM that illustrate their use for “Form,” “Fit,” and “Function.” 3. What functions can be carried out on point cloud data using reverse engineering software? How do these tools differ from conventional 3D CAD software? 4. What is your favorite term (AM, Freeform Fabrication, RP, etc.) for describing this technology and why? 5. Create a web link list of videos showing operation of different AM technologies and representative process chains.
1 Introduction and Basic Principles
6. Make a list of different characteristics of AM technologies as a means to compare with CNC machining. Under what circumstances does AM have the advantage and under what would CNC? 7. How does the Phantom desktop haptic device work and why might it be more useful for creating freeform models than conventional 3D CAD? 8. With a basic understanding of Additive Manufacturing, what is an application you can think of where additive manufacturing could be used in your daily life? Explain how. 9. What are the differences between end-use parts and prototypes? 10. What was Additive Manufacturing initially used for, and how is it utilized today? 11. Why is the term “Rapid Prototyping” not suitable for additive manufacturing anymore? 12. What is “concurrent engineering”? How can Additive Manufacturing help with concurrent engineering? 13. What type of file is typically required to use as input to process a part in an AM machine? 14. List one academic institution with research activities in AM and some of their research projects that interest you. 15. List one company which produces Additive Manufacturing machines and associated products such as materials and also list one of their products. 16. A company manufactures missile casings with internal channels. Why might Additive Manufacturing be a better manufacturing process than CNC machining? 17. Why have 3D printers not been widely applied for household use today? What benefits do you think AM will bring to your daily life in the future? 18. Visualize a process in which small robots dispersed materials in various places to construct a component. Is this an additive manufacturing process? 19. Recently historical museums have started using additive manufacturing and reverse engineering techniques. What are museums using them for? 20. Why does NASA wish to create an AM lab in outer space? 21. What changes are additive manufacturing making to the mechanical engineering field? 22. Design a product that is very difficult to make using traditional manufacturing methods but that can be printed using AM. 23. Find one Additive Manufacturing application example not covered in this book. List the benefits and disadvantages of this application compared with its traditional manufacturing method. 24. Find the newest definition for Additive Manufacturing by the ASTM F42 Committee. Make a table of all the categories of AM technologies covered in the latest standard and list one typical technique for each category. 25. Discuss how AM can improve manufacturing environmental impact and sustainability.
References 1. ASTM International (2012). Standard terminology for additive manufacturing technologies (F42 on Additive Manufacturing Technologies. Subcommittee F42. 91 on Terminology). ASTM International. 2. Burns, M. (1993). Automated fabrication: improving productivity in manufacturing. 3. Wohlers, T. (2009). Wohlers report. State of The Industry: Annual worldwide progress report. Wohlers Associates. 4. ASTM International (2015). ISO/ASTM52900–15, standard terminology for additive manufacturing – general principles – terminology. West Conshohocken: ASTM International. 5. Jacobs, P. F. (1995). Stereolithography and other RP&M technologies: from rapid prototyping to rapid tooling. Dearborn: Society of Manufacturing Engineers. 6. 3D Systems. (2020). http://www.3dsystems.com 7. Sachs, E., et al. (1992). Three dimensional printing: Rapid tooling and prototypes directly from a CAD model. Journal of Engineering for Industry, 114(4), 481–488. 8. Geomagic Reverse Engineering software. (2020). www.geomagic.com/ 9. Capture geometry inside. (2020). https://www.moldmakingtechnology.com/suppliers/cgicap 10. Bathesheba Grossman. (2020). http://www.bathsheba.com 11. Gao, Z., & Gibson, I. (2007). A 6-DOF haptic interface and its applications in CAD. International Journal of Computer Applications in Technology, 30(3), 163–170. 12. Sensable, 3D Systems. (2020). http://www.sensable.com 13. Goehrke, S. (2020). Additive Manufacturing Simulation Smartens Up In Latest ANSYS Software Release, https://www.forbes.com/sites/sarahgoehrke/2019/01/29/additive-manufacturing-simulation-smartens-up-in-latest-ansys-software-release/#1f32adad74eb
Development of Additive Manufacturing Technology
Abstract It is important to understand that AM was not developed in isolation from other technologies. It would not be possible for AM to exist were it not for innovations in areas like 3D graphics and Computer-Aided Design software. This chapter highlights some of the key moments that catalogue the development of Additive Manufacturing. It describes how the different technologies converged to a state where they could be integrated into AM machines. It will also discuss milestone AM technologies and how they have contributed to increase the range of AM applications. Furthermore, we will discuss how the application of Additive Manufacturing has evolved to include greater functionality and embrace a wider range of applications beyond the initial intent of prototyping.
2.1 Introduction Additive Manufacturing (AM) came about as a result of developments in a variety of technology sectors. Like with many manufacturing technologies, improvements in computing power and reduction in mass storage costs paved the way for processing the large amounts of data typical of modern 3D Computer-Aided Design (CAD) models within reasonable time frames. Nowadays, we have become quite accustomed to having powerful computers and other complex automated machines around us, and sometimes it may be difficult for us to imagine how the pioneers struggled to develop the first AM machines. This chapter highlights some of the key moments that catalogue the development of Additive Manufacturing technology. It will describe how the different technologies converged to a state where they could be integrated into AM machines. It will also discuss milestone AM technologies. Furthermore, we will discuss how the application of Additive Manufacturing has evolved to include greater functionality and embrace a wider range of applications beyond the initial intention of just proto© Springer Nature Switzerland AG 2021 I. Gibson et al., Additive Manufacturing Technologies, https://doi.org/10.1007/978-3-030-56127-7_2
2 Development of Additive Manufacturing Technology
typing. We close the chapter with a summary of standards that have been developed to support the adoption of AM.
2.2 Computers Like many other technologies, AM came about as a result of the invention of the computer. However, there was little indication that the first computers built in the 1940s (like the Zuse Z3 , ENIAC , and EDSAC  computers) would change lives in the way that they so obviously have. Inventions like the thermionic valve, transistor, and microchip made it possible for computers to become faster, smaller, and cheaper with greater functionality. This development has been so quick that even Bill Gates of Microsoft was caught off guard when he thought in 1981 that 640 kb of memory would be sufficient for any Windows-based computer. In 1989, he admitted his error when addressing the University of Waterloo Computer Science Club . Similarly in 1977, Ken Olsen of Digital Electronics Corp. (DEC) stated that there would never be any reason for people to have computers in their homes when he addressed the World Future Society in Boston . That remarkable misjudgment may have caused Olsen to lose his job not long afterward. One key to the development of computers as serviceable tools lies in their ability to perform tasks in real time. In the early days, serious computational tasks took many hours or even days to prepare, run, and complete. This served as a limitation to everyday computer use, and it is only since it was shown that tasks can complete in real time that computers have been accepted as everyday items rather than just for academics or big business. This has included the ability to display results not just numerically but graphically as well. For this we owe a debt of thanks at least in part to the gaming industry, which has pioneered many developments in graphics technology with the aim to display more detailed and more “realistic” images to enhance the gaming experience. AM takes full advantage of many of the important features of computer technology, both directly (in the AM machines themselves) and indirectly (within the supporting technology), including: • Processing power: Part data files can be very large and require a reasonable amount of processing power to manipulate while setting up the machine and when slicing the data before building. Earlier machines would have had difficulty handling large CAD data files. • Graphics capability: AM machine operation does not require a big graphics engine except to see the file while positioning within the virtual machine space. However, all machines benefit from a good graphical user interface (GUI) that can make the machine easier to set up, operate, and maintain. • Machine control: AM technology requires precise positioning of equipment in a similar way to a Computer Numerical Controlled (CNC) machining center or even a high-end photocopy machine or laser printer. Such equipment requires controllers that take information from sensors for determining status and actuators for positioning and other output functions. Computation is generally required
in order to determine the control requirements. Conducting these control tasks even in real time does not normally require significant amounts of processing power by today’s standards. Dedicated functions like positioning of motors, lenses, etc. would normally require individual controller modules. A computer would be used to oversee the communication to and from these controllers and pass data related to the part build function. • Networking: Nearly every computer these days has a method for communicating with other computers around the world. Files for building would normally be designed on another computer to that running the AM machine. Earlier systems would have required the files to be loaded from disk or tape. Nowadays almost all files will be sent using an Ethernet connection, often via the Internet. • Integration: As is indicated by the variety of functions, the computer forms a central component that ties different processes together. The purpose of the computer would be to communicate with other parts of the system, to process data, and to send that data from one part of the system to the other. Figure 2.1 shows how the abovementioned technologies are integrated to form an AM machine. Earlier computer-based design environments required physically large mainframe and mini computers. Workstations that generally ran the graphics and input/ output functions were connected to these computers. The computer then ran the complex calculations for manipulating the models. This was a costly solution based around the fact that the processor and memory components were very expensive elements. With the reduction in the cost of these components, personal computers Actuators
Environmental control temperature, humidity, atmosphere, etc.
Interlayer control, recoating, head cleaning ,etc.
Z control for platform movement
XY control for layer plotting
Internet Process setup
Fig. 2.1 General integration of an AM machine
2 Development of Additive Manufacturing Technology
(PCs) became viable solutions. Earlier PCs were not powerful enough to replace the complex functions that workstation-based computers could perform, but the speedy development of PCs soon overcame all but the most computationally expensive requirements. Without computers there would be no capability to display 3D graphic images. Without 3D graphics, there would be no 3D Computer-Aided Design. Without this ability to represent objects digitally in 3D, we would have a limited desire to use machines to fabricate anything but the simplest shapes. It is safe to say, therefore, that without the computers we have today, we would not have seen Additive Manufacturing develop.
2.3 Computer-Aided Design Technology Today, every engineering student must learn how to use computers for many of their tasks, including the development of new designs. CAD technologies are available for assisting in the design of large buildings and of nano-scale microprocessors. CAD technology holds within it the knowledge associated with a particular type of product, including geometric, electrical, thermal, dynamic, and static behavior. CAD systems may contain rules associated with such behaviors that allow the user to focus on design and functionality without worrying too much whether a product can or cannot work. CAD also allows the user to focus on small features of a large product, maintaining data integrity and ordering it to understand how subsystems integrate with the remainder. Additive Manufacturing technology primarily makes use of the output from 3D solid modeling CAD software. It is important to understand that this is only a branch of a much larger set of CAD systems and, therefore, not all CAD systems will produce output suitable for layer-based AM technology. Currently, AM technology focuses on reproducing geometric form, and so the better CAD systems to use are those that produce such forms in the most precise and effective way. Early CAD systems were extremely limited by the display technology. The first display systems had little or no capacity to produce anything other than alphanumeric text output. Some early computers had specialized graphic output devices that displayed graphics separate from the text commands used to drive them. Even so, the geometric forms were shown primarily in a vector form, displaying wire-frame output. As well as the heavy demand on the computing power required to display the graphics for such systems, this was because most displays were monochrome, making it very difficult to show 3D geometric forms on screen without lighting and shading effects. CAD would not have developed so quickly if it were not for the demands set by computer-aided manufacturing (CAM). CAM represents a channel for converting the virtual models developed in CAD into the physical products that we use in our everyday lives. It is doubtful that without the demands associated with this conversion from virtual to real that CAD would have developed so far or so quickly. This,
2.3 Computer-Aided Design Technology
in turn, was fueled and driven by the developments in associated technologies, like processor, memory, and display technologies. CAM systems produce the code for numerically controlled (NC) machinery, essentially combining coordinate data with commands to select and actuate the cutting tools. Early NC technologies would take CAM data relating to the location of machined features, like holes, slots, pockets, etc. These features would then be fabricated by machining from a stock material. As NC machines proved their value in their precise, automated functionality, so the sophistication of the features increased. This has now extended to the ability to machine highly complex, freeform surfaces. However, there are two key limitations to all NC machining: • Almost every part must be made in stages, often requiring multiple passes for material removal and setups. • All machining is performed from an approach direction (sometimes referred to as 2.5D rather than fully 3D manufacture). This requires that the stock material be held in a particular orientation and that not all the material can be accessible at any one stage in the process. NC machining, therefore, only requires surface modeling software. All early CAM systems were based on surface modeling CAD. AM technology was the first automated computer-aided manufacturing process that truly required 3D solid modeling CAD. It was necessary to have a fully enclosed surface to generate the driving coordinates for AM. This can be achieved using surface modeling systems, but because surfaces are described by boundary curves, it is often difficult to precisely and seamlessly connect these together. Even if the gaps are imperceptible, the resulting models may be difficult to build using AM. At the very least, any inaccuracies in the 3D model would be passed on to the AM part that was constructed. Early AM applications often displayed difficulties because of associated problems with surface modeling software. Since it is important for AM systems to have accurate models that are fully enclosed, the preference is for solid modeling CAD. Solid modeling CAD ensures that all models made have a volume and, therefore, by definition are fully enclosed surfaces. While surface modeling can be used in part construction, we cannot always be sure that the final model is faithfully represented as a solid. Such models are generally necessary for computer-aided engineering (CAE) tools like finite element analysis (FEA) but are also very important for other CAM processes. Most CAD systems can now quite readily run on PCs. This is generally a result of the improvements in computer technology mentioned earlier but is also a result in improvements in the way CAD data is presented, manipulated, and stored. Most CAD systems utilize non-uniform rational basis splines or NURBS . NURBS are an excellent way of precisely defining the curves and surfaces that correspond to the outer shell of a CAD model. Since model definitions can include freeform surfaces as well as simple geometric shapes, the representation must accommodate this, and splines are complex enough to represent such shapes without making the files too large and unwieldy. They are also easy to manipulate to modify the resulting shape. CAD technology has rapidly improved along the following lines:
2 Development of Additive Manufacturing Technology
• Realism: With lighting, shading effects, ray tracing, and other photorealistic imaging techniques, it is becoming possible to generate images of the CAD models that are difficult to distinguish from actual photographs. In some ways, this reduces the requirements on AM models for visualization purposes. • Usability and user interface: Early CAD software required the input of text- based instructions through a dialog box. Development of Windows-based graphical user interfaces (GUIs) has led to graphics-based dialogs and even direct manipulation of models within virtual 3D environments. Instructions are issued through the use of drop-down menu systems and context-related commands. To suit different user preferences and styles, it is often possible to execute the same instruction in different ways. Keyboards are still necessary for input of specific measurements, but the usability of CAD systems has improved dramatically. There is still some way to go to make CAD systems available to those without engineering knowledge or without training, however. • Engineering content: Since CAD is almost an essential part of a modern engineer’s training, it is vital that the software includes as much engineering content as possible. With solid modeling CAD, it is possible to calculate the volumes and masses of models, to investigate fits and clearances according to tolerance variations, and to export files with mesh data for finite element analysis. FEA is often even possible without having to leave the CAD system. • Speed: As mentioned previously, the use of NURBS assists in optimizing CAD data manipulation. CAD systems are constantly being optimized in various ways, mainly by exploiting the hardware developments of computers. • Accuracy: If high tolerances are expected for a design, then it is important that calculations are precise. High precision can make heavy demands on processing time and memory. • Complexity: All of the above characteristics can lead to extremely complex systems. It is a challenge to software vendors to incorporate these features without making them unwieldy and unworkable. • Usability: Recent developments in CAD technology have focused on making the systems available to a wider range of users. In particular the aim has been to allow untrained users to be able to design complex geometry parts for themselves. There are now 3D solid modeling CAD systems that run entirely within a web browser with similar capabilities to workstation systems of only 10 years ago. Many CAD software vendors are focusing on producing highly integrated design environments that allow designers to work as teams and to share designs across different platforms and for different departments. Industrial designers must work with sales and marketing, engineering designers, analysts, manufacturing engineers, and many other branches of an organization to bring a design to fruition as a product. Such branches may even be in different regions of the world and may be part of the same organization or acting as subcontractors. The Internet must therefore also be integrated with these software systems, with appropriate measures for fast and accurate transmission and protection of intellectual property.
2.3 Computer-Aided Design Technology
Fig. 2.2 A CAD model on the left converted into STL format on the right
It is quite possible to directly manipulate the CAD file to generate the slice data that will drive an AM machine, and this is commonly referred to as direct slicing . However, this would mean every CAD system must have a direct slicing algorithm that would have to be compatible with all the different types of AM technology. Alternatively, each AM system vendor would have to write a routine for every CAD system. Both of these approaches are impractical. The solution is to use a generic format that is specific to the technology. This generic format was developed by 3D Systems, USA, who was the first company to commercialize AM technology and called the file format “STL” after their stereolithography technology (an example of which is shown in Fig. 2.2). The STL file format was made public domain to allow all CAD vendors to access it easily and hopefully integrate it into their systems. This strategy has been successful, and STL is now a standard output for nearly all solid modeling CAD systems and has also been adopted by AM system vendors . STL uses triangles to describe the surfaces to be built. Each triangle is described as three points and a facet normal vector indicating the outward side of the triangle, in a manner similar to the following: facet normal − 4.470293E−02 7.003503E−01 − 7.123981E-01, outer loop, vertex − 2.812284E+00 2.298693E+01 0.000000E+00, vertex − 2.812284E+00 2.296699E+01–1.960784E−02, vertex − 3.124760E+00 2.296699E+01 0.000000E+00, endloop, endfacet. The demands on CAD technology in the future are set to change with respect to AM. As we move toward more and more functionality in the parts produced by AM, we must understand that the CAD system must include rules associated with AM. To date, the focus has been on the external geometry. In the future, we may need to know rules associated with how the AM systems function so that the output can be optimized.
2 Development of Additive Manufacturing Technology
2.4 Other Associated Technologies Aside from computer technology, there are a number of other technologies that have developed along with AM that are worthy of note here since they have served to contribute to further improvement of AM systems.
2.4.1 Printing Technologies Inkjet and droplet printing technologies have rapidly developed in recent years. Improvements in resolution and reduction in costs has meant that high-resolution printing, typically with multiple colors, is available as part of our everyday lives. Such improvement in resolution has also been supported by improvement in material handling capacity and reliability. Initially, colored inks were low viscosity and fed into the print heads at ambient temperatures. Now it is possible to generate much higher pressures within the droplet formation chamber so that materials with much higher viscosity and even molten materials can be printed. This means that droplet deposition can now be used to print photocurable and molten resins as well as binders for powder systems. Since print heads are relatively compact devices with all the droplet control technology highly integrated into these heads (like the one shown in Fig. 2.3), it is possible to produce low-cost, high-resolution, high- throughput AM technology.
Y axis UV light Fullcure M
Fig. 2.3 Printer technology used on an AM machine. (Photo courtesy of Objet)
2.4 Other Associated Technologies
2.4.2 Programmable Logic Controllers The input CAD models for AM are large data files generated using standard computer technology. Once they are on the AM machine, however, these files are reduced to a series of process stages that require sensor input and signaling of actuators. This process and machine control is often best carried out using microcontroller systems rather than microprocessor systems. Industrial microcontroller systems form the basis of programmable logic controllers (PLCs), which are used to reliably control industrial processes. Designing and building industrial machinery, like AM machines, are much easier using building blocks based around modern PLCs for coordinating and controlling the various steps in the machine process.
2.4.3 Materials Early AM technologies were built around materials that were already available and that had been developed to suit other processes. However, AM processes are somewhat unique, and these original materials were far from ideal for these new applications. For example, the early photocurable resins resulted in models that were brittle and that warped easily. Powders used in Laser-Based Powder Bed Fusion (LB-PBF) processes degraded quickly within the machine, and many of the materials resulted in parts that were quite weak. As we came to understand the technology better, materials were developed specifically to suit AM processes. Materials have been tuned to suit more closely the operating parameters of the different processes and to provide better output parts. As a result, parts are now much more accurate, stronger, and longer lasting. In turn, these new materials have resulted in the processes being tuned to produce higher-temperature materials (including metals), smaller feature sizes, and faster throughput.
2.4.4 Computer Numerically Controlled Machining One of the reasons AM technology was originally developed was because CNC technology was not able to produce satisfactory output within the required time frames. CNC machining was slow, cumbersome, and difficult to operate. AM technology on the other hand was quite easy to set up with quick results but had poor accuracy and limited material capability. As improvements in AM technologies came about, vendors of CNC machining technology realized that there was now growing competition. CNC machining has dramatically improved, just as AM technologies have matured. It could be argued that high-speed CNC would have developed anyway, but some have argued that the perceived threat from AM technology caused CNC machining vendors to rethink how their machines were made. The combination of high-speed machining and AM for certain applications, such as for
2 Development of Additive Manufacturing Technology
3D Printed mold insert
Machined mold base
Fig. 2.4 Standardized mold system and 3D printed mold inserts permitting rapid, low-cost prototypes. (Photo courtesy of HASCO) 
making large, complex, and durable molds for standardized mold system (plastic injection molding), as shown in Fig. 2.4 , illustrates how the two can be used interchangeably to take advantage of the benefits of both technologies. For geometries that can be machined using a single setup orientation, CNC machining is often the fastest, most cost-effective method. For parts with complex geometries or parts which require a large proportion of the overall material volume to be machined away as scrap, AM can be used to more quickly and economically produce the part than when using CNC.
2.5 The Use of Layers A key enabling principle of AM part manufacture is the use of layers as finite 2D cross-sections of the 3D model. Almost every AM technology builds parts using layers of material added together, primarily due to the simplification of building 3D objects. Using 2D representations to represent cross-sections of a more complex 3D feature has been common in many applications outside AM. The most obvious example of this is how cartographers use a line of constant height to represent hills and other geographical reliefs. These contour lines, or iso-heights, can be used as plates that can be stacked to form representations of geographical regions. The gaps between these 2D cross-sections cannot be precisely represented and are therefore approximated, or interpolated, in the form of continuity curves connecting these layers. Such techniques can also be used to provide a 3D representation of other physical properties, like isobars or isotherms on weather maps. Architects have also used such methods to represent landscapes of actual or planned areas, like that used by an architect firm in Fig. 2.5 . The concept is
2.6 Classification of AM Processes
Fig. 2.5 An architectural landscape model, illustrating the use of layers. (Photo courtesy of LiD)
particularly logical to manufacturers of buildings who also use an additive approach, albeit not using layers. Consider how the pyramids in Egypt and in South America were created. Notwithstanding how they were fabricated, it’s clear that they were created using a layered approach, adding material as they went.
2.6 Classification of AM Processes There are numerous ways to classify AM technologies. A popular approach is to classify according to baseline technology, like whether the process uses lasers, printer technology, extrusion technology, etc. [12, 13]. Another approach is to collect processes together according to the type of raw material input [14, 15]. The problem with these classification methods is that some processes get lumped together in what seems to be odd combinations (like Selective Laser Sintering being grouped together with 3D Printing) or that some processes that may appear to produce similar results end up being separated (like stereolithography and material jetting (MJT) with photopolymers). It is probably inappropriate, therefore, to use a single classification approach. An early classification method was described by Pham , which uses a two- dimensional classification method as shown in Fig. 2.6. The first dimension relates to the method by which the layers are constructed. Earlier technologies used a single point source to draw across the surface of the base material. Later systems increased the number of sources to increase the throughput, which was made possible with the use of droplet deposition technology, for example, which can be constructed into a one-dimensional array of deposition heads. Further throughput improvements are possible with the use of 2D array technology using the likes of digital micromirror devices (DMDs) and high-resolution display technology, capable of exposing an entire surface in a single pass. However, just using this classifica-
2 Development of Additive Manufacturing Technology
1D Channel Y X
2×1D Channels Y1
Array of 1D Channels
SLA (3D Sys)
SLA (3D Sys) LST (EOS), LENS Phonix, SDM
Solido PLT (KIRA)
Dual beam SLA (3DSys)
Envisiontech Micro TEC
Fig. 2.6 Layered manufacturing (LM) processes as classified by Pham (note that this diagram has been amended to include some recent AM technologies)
tion results in the previously mentioned anomalies where numerous dissimilar processes are grouped together. This is solved by introducing a second dimension of raw material to the classification. Pham uses four separate material classifications: liquid polymer, discrete particles, molten material, and laminated sheets. Some more exotic systems mentioned in this book may not fit directly into this classification. An example is the possible deposition of composite material, like concrete, using an extrusion-based technology. This fits well as a 1D channel, but the material is not explicitly listed as it is not really a molten material. Furthermore, future systems may be developed that use 3D holography to project and fabricate complete objects in a single pass. As with many classifications, there can sometimes be processes or systems that lie outside them. If there are sufficient systems to warrant an extension to this classification, then it should not be a problem. It should be noted that, in particular, 1D and 2 × 1D channel systems combine both vector- and raster-based scanning methods. Often, the outline of a layer is traced first before being filled in with regular or irregular scanning patterns. The outline is generally referred to as vector scanned, while the fill pattern can often be generalized as a raster pattern. The array methods tend not to separate the outline and the fill. Most AM technology started using a 1D channel approach, although one of the earliest and now obsolete technologies, Solid Ground Curing from Cubital, used liquid photopolymers and essentially (although perhaps arguably) a 2D channel method. As technology developed, so more of the boxes in the classification array began to be filled. The empty boxes in this array may serve as a guide to researchers and developers for further technological advances. Most of the 1D array methods use at least 2 × 1D lines. This is similar to conventional 2D printing where each line deposits a different material in different locations within a layer. The Connex pro-
2.6 Classification of AM Processes
cess using the PolyJet technology from Stratasys is a good example of this where it is possible to create parts with different material properties in a single step using this approach. Color 3D Printing is possible using multiple 1D arrays with ink or separately colored material in each. Note however that the part coloration in the sheet laminating Mcor process  is separated from the layer formation process, which is why it is defined as a 1D channel approach.
2.6.1 Liquid Polymer Systems As can be seen from Fig. 2.6, liquid polymers appear to be a popular material. The first commercial system was the 3D Systems Stereolithography process based on liquid photopolymers. A large portion of systems in use today are, in fact, not just liquid polymer systems but more specifically liquid photopolymer systems. However, this classification should not be restricted to just photopolymers, since a number of experimental systems are using hydrogels that would also fit into this category. Furthermore, the [email protected] system developed at Cornell University in the USA and the open-source RepRap systems originating from Bath University in the UK also use liquid polymers with curing techniques other than UV or other wavelength optical curing methods [18, 19]. Using this material and a 1D channel or 2 × 1D channel scanning method, a great option is to use a laser like in the stereolithography process. Droplet deposition of polymers using an array of 1D channels can simplify the curing process to a floodlight (for photopolymers) or similar method. This approach was commercialized by the Israeli company Objet (now part of Stratasys) who use printer technology to print fine droplets of photopolymer “ink” . One unique feature of the Objet system is the ability to vary the material properties within a single part. Parts can, for example, have soft-feel, rubber-like features combined with more solid resins to achieve a result similar to an overmolding effect. Controlling the area to be exposed using digital micromirror devices or other highresolution display technology obviates the need for any scanning at all, thus increasing throughput and reducing the number of moving parts. DMDs are generally applied to micron-scale additive approaches, like those used by Microtec in Germany . For normal-scale systems, EnvisionTEC uses high-resolution DMD displays to cure photopolymer resin in their low-cost AM machines. The 3D Systems V-Flash process is also a variation on this approach, exposing thin sheets of polymer spread onto a build surface.
2.6.2 Discrete Particle Systems Discrete particles are normally powders that are generally graded into a relatively uniform particle size and shape and narrow size distribution. The finer the particles, the better, but there will be problems if the dimensions get too small in terms of
2 Development of Additive Manufacturing Technology
controlling the distribution and dispersion. Again, the conventional 1D channel approach is to use a laser, this time to produce thermal energy in a controlled manner and, therefore, raise the temperature sufficiently to melt the powder. Polymer powders must therefore exhibit thermoplastic behavior so that they can be melted and remelted to permit bonding of one layer to another. There are a wide variety of such systems that generally differ in terms of the material that can be processed. The two main polymer-based systems commercially available are the Selective Laser Sintering (SLS) technology marketed by 3D Systems  and the EOSINT processes developed by the German company EOS . Application of printer technology to powder beds resulted in the (original) 3D Printing (3DP) process. This technique was developed by researchers at MIT in the USA . Droplet printing technology is used to print a binder, or glue, onto a powder bed. The glue sticks the powder particles together to form a 3D structure. This basic technique has been developed for different applications dependent on the type of powder and binder combination. The most successful approaches use low- cost, starch-, and plaster-based powders with inexpensive glues, as commercialized by Z Corp, USA , which is now part of 3D Systems. Ceramic powders and appropriate binders were similarly used in the Direct Shell Production Casting (DSPC) process by Soligen  as part of a service to create shells for casting of metal parts. Alternatively, if the binder were to contain an amount of drug, 3DP can be used to create controlled delivery-rate drugs like in the process developed by the US company Therics. Neither of these last two processes has proven to be as successful as that licensed by Z Corp/3D Systems. One particular advantage of the Z Corp technology is that the binders can be jetted from multi-nozzle print heads. Binders coming from different nozzles can be different, and, therefore, subtle variations can be incorporated into the resulting part. The most obvious of these is the color that can be incorporated into parts.
2.6.3 Molten Material Systems Molten material systems are characterized by a preheating chamber that raises the material temperature to the melting point so that it can flow through a delivery system. The most well-known method for doing this is the Fused Deposition Modeling (FDM) Material Extrusion (MEX) technology developed by the US company Stratasys . This approach extrudes the material through a nozzle in a controlled manner. Two extrusion heads are often used so that support structures can be fabricated from a different material to facilitate part cleanup and removal. It should be noted that there are now a huge number of variants of this technology due to the lapse of key FDM patents. This competition has driven the price of these machines down to such a level that individual buyers can afford to have their own machines at home. Printer technology has also been adapted to suit this material delivery approach. One technique, developed initially as the Sanders prototyping
2.6 Classification of AM Processes
machine, that later became Solidscape, USA , and which is now part of Stratasys, is a 1D channel system. A single jet piezoelectric deposition head lays down wax material. Another head lays down a second wax material with a lower melting temperature that is used for support structures. The droplets from these print heads are very small so the resulting parts are fine in detail. To further maintain the part precision, a planar cutting process is used to level each layer once the printing has been completed. Supports are removed by inserting the complete part into a temperature-controlled bath that melts the support material away, leaving the part material intact. The use of wax along with the precision of Solidscape machines makes this approach ideal for precision casting applications like jewelry, medical devices, and dental castings. Few machines are sold outside of these niche areas. The 1D channel approach, however, is very slow in comparison with other methods, and applying a parallel element does significantly improve throughput. The Thermojet technology from 3D Systems also deposits a wax material through droplet-based printing heads. The use of parallel print heads as an array of 1D channels effectively multiplies the deposition rate. The Thermojet approach, however, is not widely used because wax materials are difficult and fragile when handled. Thermojet machines are no longer being made, although existing machines are commonly used for investment casting patterns.
2.6.4 Solid Sheet Systems One of the earliest AM technologies was the Laminated Object Manufacturing (LOM) system from Helisys, USA. This technology used a laser to cut out profiles from sheet paper, supplied from a continuous roll, which formed the layers of the final part. Layers were bonded together using a heat-activated resin that was coated on one surface of the paper. Once all the layers were bonded together, the result was very like a wooden block. A hatch pattern cut into the excess material allowed the user to separate away waste material and reveal the part. A similar approach was used by the Japanese company Kira, in their Solid Center machine , and by the Israeli company Solidimension with their Solido machine. The major difference is that both these machines cut out the part profile using a blade similar to those found in vinyl sign-making machines, driven using a 2D plotter drive. The Kira machine used a heat-activated adhesive applied using laser printing technology to bond the paper layers together. Both the Solido and Kira machines have been discontinued for reasons including poor reliability, material wastage, and the need for excessive amounts of manual post-processing. Mcor Technologies expanded upon this approach and produces a modern version of this technology, using low-cost color printing to make it possible to make laminated color parts .
2 Development of Additive Manufacturing Technology
2.6.5 New AM Classification Schemes In this book, we use a version of Pham’s classification introduced in Fig. 2.6. Instead of using the 1D and 2 × 1D channel terminology, we will typically use the terminology “point” or “point-wise” systems. For arrays of 1D channels, such as when using inkjet print heads, we refer to this as “line” processing. 2D channel technologies will be referred to as “layer” processing. Last, although no current commercialized processes are capable of this, holographic-like techniques are considered “volume” processing. The technology-specific descriptions starting in Chap. 4 are based, in part, upon a separation of technologies into groups where processes which use a common type of machine architecture and similar materials transformation physics are grouped together. This grouping is a refinement of an approach introduced by Stucker and Janaki Ram in the CRC Materials Processing Handbook . In this grouping scheme, for example, processes which use a common machine architecture developed for stacking layers of powdered material and a materials transformation mechanism using heat to fuse those powders together are all discussed in the PBF chapter. These are grouped together even though these processes encompass polymer, metal, ceramic, and composite materials, multiple types of energy sources (e.g., lasers and infrared heaters), and point-wise and layer processing approaches. Using this classification scheme, all AM processes fall into one of seven categories. An understanding of these seven categories should enable a person familiar with the concepts introduced in this book to quickly grasp and understand an unfamiliar AM process by comparing its similarities, benefits, drawbacks, and processing characteristics to the other processes in the grouping into which it falls. This classification scheme from the first edition of this textbook had an important impact on the development and adoption of ASTM/ISO standard terminology. The authors were involved in these consensus standards activities, and we have agreed to adopt the modified terminology from ASTM F42 and ISO TC 261 in the second and subsequent editions . Of course, in the future, we will continue to support the ASTM/ISO standardization efforts and keep the textbook up to date. The seven process categories are presented here. Chapters 4, 5, 6, 7, 8, 9, and 10 cover each one in detail: • Vat Photopolymerization (VPP): processes that utilize a liquid photopolymer that is contained in a vat and processed by selectively delivering energy to cure specific regions of a part cross-section. • Powder Bed Fusion (PBF): processes that utilize a container filled with powder that is processed selectively using an energy source, most commonly a scanning laser or electron beam. • Material Extrusion (MEX): processes that deposit a material by extruding it through a nozzle, typically while scanning the nozzle in a pattern that produces a part cross-section. • Material Jetting (MJT): processes that selectively deposit droplets of feedstock material.
2.7 Heat Sources
• Binder Jetting (BJT): processes where a liquid bonding agent is printed into a powder bed in order to form part cross-sections. • Sheet Lamination (SHL): processes that bond sheets of material to form a part. • Directed Energy Deposition (DED): processes that simultaneously deposit a material (usually powder or wire) and provide energy to process that material through a single deposition device.
2.7 Heat Sources 2.7.1 Lasers Many of the earliest AM systems were based on laser technology. The reasons are that lasers provide a high intensity and highly collimated beam of energy that can be moved very quickly in a controlled manner with the use of directional mirrors. Since AM requires the material in each layer to be solidified or joined in a selective manner, lasers are ideal candidates for use, provided the laser energy is compatible with the material transformation mechanisms. There are two kinds of laser processing used in AM: curing and heating. With photopolymer resins the requirement is for laser energy of a specific frequency that will cause the liquid resin to solidify or “cure.” Usually this laser is in the ultraviolet range, but other frequencies can be used. For heating, the requirement is for the laser to carry sufficient thermal energy to cut through a layer of solid material, to cause powder to melt, or to cause sheets of material to fuse. For powder processes, for example, the key is to melt the material in a controlled fashion without creating too great a buildup of heat, so that when the laser energy is removed, the molten material rapidly solidifies again. For cutting, the intention is to separate a region of material from another in the form of laser cutting. Earlier AM machines used tube lasers to provide the required energy, but most manufacturers have switched to solid-state technology, which provides greater efficiency, lifetime, and reliability. A laser generally has the following components: (I) gain medium, (II) a pumping energy source, and (III) optical resonator. The gain medium is located in the optical resonator and amplifies the light beam by stimulating emission. Lasers are classified according to the type of gain medium. Figure 2.7 shows the classification of lasers.
Solid State Fig. 2.7 Different lasers
Fiber or semiconductors
2 Development of Additive Manufacturing Technology
In Additive Manufacturing gas, solid-state and fiber lasers are the most commonly used. Early AM machines used gas lasers, primarily CO2. The most common gas lasers produce infrared output wavelengths ranging from 9000 to 11,000 nm with an efficiency of 5–20% and power ranging from 100 to 20,000 W. The simplicity of a gas laser system brings low cost, highly reliability, and system compactness, which are the main reasons that CO2 lasers are the workhorse of precision manufacturing. However, their output power is relatively non-stable because of thermal expansion and contraction of the laser structure due to the heat generated in the process of energy pumping to a large volume of CO2 gas. Low light absorption in the infrared region is another problem of CO2 lasers, with high reflectivity among metals in particular. Nd:YAG is a solid-state laser, and the gain medium is made of rod-shaped Nd:YAG crystals. The gain medium is pumped by a flash lamp or 808 nm laser diode to produce a near-infrared output wavelength of 1064 nm. The significant advantages of this laser over CO2 are system compactness and efficiency in delivering the beam through optical fibers. This laser can be operated both in continuous mode using crystals doped with low concentrations and in pulsed mode using highly doped crystals. The maximum output power for continuous and pulse lasers is a few kW and 20 kW, respectively. This laser suffers from relatively low electrical-tooptical power conversion efficiency which leads to lower beam quality. The reason is most of the unabsorbed energy is dissipated as heat. This heat leads to thermal lensing and poor beam quality. Diode-pumped solid-state (DPSS) lasers are a solution for these problems. The gain medium for fiber lasers is made from rare earth-doped optical fibers such as Yb-fibers. This fiber has high quantum efficiency (−95%). They can produce a near-infrared laser beam in the range 1030–1070 nm output wavelength and have high electrical-to-optical efficiency (−25%), excellent beam quality, robustness against environmental disturbances, and system compactness. Light propagation inside the fiber, unexpected polarization change from fiber bending, vibration, and temperature variation are typical problems of Yb-fiber lasers. Excited dimer (Excimers) are gas mixtures containing a noble gas (e.g., argon, krypton, or xenon), a halogen (e.g., fluorine or chlorine), and a buffer gas (typically neon or helium). If the gain medium is made by excimers, the system is called an excimer laser. In this laser nanosecond pulses in the ultraviolet region are produced by pumping excimers using pulsed electrical discharge. The wavelength of excimers is in the range of 157–351 nm, and average output power can go up to a few hundreds of Watts. Most materials have a high absorptivity in the UV region, which is a significant advantage. Disadvantages of this laser are poor beam quality, high maintenance, and high running cost.
2.7 Heat Sources
2.7.2 Electron Beam An electron beam is another energy source used to melt materials in Additive Manufacturing. In this method free electrons in a vacuum can be controlled and positioned by electric and magnetic fields to shape a beam. When a high-velocity beam of electrons contacts solid matter, the kinetic energy is transformed to heat. This high heat, when concentrated, is an efficient means for melting materials that are electrically conductive. Electron beams require a vacuum chamber, since electrons scatter and diffuse if they interact with gas atoms between the electron gun and the material being heated. Electron beam melting (EBM) has a higher production rate compared to laser beam melting due to a higher energy density. A greater energy density leads to Marangoni convection in the melting area, which results in lower surface quality (roughness) and thus higher dimensional deviations. More Additive Manufacturing machines are equipped with lasers than electron beams.
2.7.3 Electric Arc/Plasma Arc The electrical breakdown of a gas in a nonconductive medium like air produces plasma and an electric arc, plasma arc, or arc discharge. A normal gas molecule at room temperature consists of two or more atoms. When the temperature of the molecule increases to 2000 °C, atoms are separated. If the gas temperature goes up to 3000 °C, some of the atoms are separated, and gas is ionized and decomposition of atoms happens. This gas is called plasma and is a conductor of electricity, and so plasma is the fourth state of matter. The plasma is accompanied by electrical discharge. The source of heat production in plasma is the recombination of electrons and ions to form atoms and the recombining of atoms to form molecules. This released bonding energy increases the kinetic energy of atoms or molecules formed by recombination and can be used in different material processing. This temperature can go up to 30,000 °C and be used for melting and evaporation of almost all materials. Electrical and plasma arcs are used in Additive Manufacturing mainly in Directed Energy Deposition (DED) using wire. This is also referred to as Wire Arc Additive Manufacturing (WAAM). In WAAM motion can be provided either by robotic systems or Computer Numerical Controlled gantries. In this method wire plays the role of a consumable electrode . Electrical or plasma arcs are used particularly for building large components due to their high deposition rate, low material and equipment costs, and good structural integrity. These specifications characterize it as a suitable candidate for replacing the conventional methods of manufacturing from solid billets or large forgings, notably with regard to low and medium complexity parts.
2 Development of Additive Manufacturing Technology
2.8 Metal Systems One of the most important historical developments in AM was the proliferation of direct metal processes. Machines like the EOSINT-M  and Laser Engineered Net Shaping (LENS) have been around for a number of years [33, 34]. Recent additions from other companies and improvements in laser technology, machine accuracy, speed, and cost have opened up this market, and today, metal AM is a major driver of AM adoption. Most direct metal systems work using a point-wise method, and nearly all of them utilize metal powders as input. The main exception to this approach is the Sheet Lamination (SHL) processes, particularly the Ultrasonic Consolidation process commercialized by Solidica, USA (now Fabrisonic), which uses sheet metal laminates that are ultrasonically welded together . Of the powder systems, almost every newer machine uses a powder spreading approach similar to the Selective Laser Sintering process, followed by melting using an energy beam. This energy is normally a high-power laser, except in the case of the EBM process by the Swedish company Arcam  (now part of GE). Another approach is the LENS powder delivery system used by Optomec . This machine employs powder delivery through a nozzle placed above the part. The powder is melted where the material converges with the laser and the substrate. This approach allows the process to be used to add material to an existing part, which means it can be used for repair of expensive metal components that may have been damaged, like chipped turbine blades and injection mold tool inserts.
2.9 Hybrid Systems Some of the machines described above are, in fact, hybrid additive/subtractive processes rather than purely additive. Including a subtractive component can assist in making the process more precise. An example is the use of planar milling at the end of each additive layer in the Sanders and Objet machines. This stage makes for a smooth planar surface onto which the next layer can be added, negating cumulative effects from errors in droplet deposition height. It should be noted that when subtractive methods are used, waste will be generated. Machining processes require removal of material that in general cannot easily be recycled. Similarly, many additive processes require the use of support structures, and these too must be removed or “subtracted.” It can be said that with the Objet process, for instance, the additive element is dominant and that the subtractive component is important but relatively insignificant. There have been a number of attempts to merge subtractive and additive technologies together where the subtractive component is the dominant element. An excellent example of this is the Stratoconception approach , where the original CAD models are divided into thick machinable layers. Once these layers are
2.10 Milestones in AM Development
machined, they are bonded together to form the complete solid part. This approach works very well for very large parts that may have features that would be difficult to machine using a multi-axis machining center due to the accessibility of the tool. This approach can be applied to foam- and wood-based materials or to metals. For structural components it is important to consider the bonding methods. For high- strength metal parts, diffusion bonding may be an alternative. A lower-cost solution that works in a similar way is Subtractive RP (SRP) from Roland , who is also famous for plotter technology. SRP makes use of Roland desktop milling machines to machine sheets of material that can be sandwiched together, similar to Stratoconception. The key is to use the exterior material as a frame that can be used to register each slice to others and to hold the part in place. With this method not all the material is machined away, and a web of connecting spars are used to maintain this registration. Another variation of this method that was never commercialized was Shape Deposition Manufacturing (SDM), developed mainly at Stanford and Carnegie- Mellon Universities in the USA . With SDM, the geometry of the part is devolved into a sequence of easier to manufacture parts that can in some way be combined together. A decision is made concerning whether each subpart should be manufactured using additive or subtractive technology dependent on such factors as the accuracy, material, geometrical features, functional requirements, etc. Furthermore, parts can be made from multiple materials, combined together using a variety of processes, including the use of plastics, metals, and even ceramics. Some of the materials can also be used in a sacrificial way to create cavities and clearances. Additionally, the “layers” are not necessarily planar, nor constant in thickness. Such a system would be unwieldy and difficult to realize commercially, but the ideas generated during this research have influenced many studies and systems thereafter. In this book, for technologies where both additive and subtractive approaches are used, these technologies are discussed in the chapter where their additive approach best fits.
2.10 Milestones in AM Development We can look at the historical development of AM in a variety ways. The origins may be difficult to properly define, and there was certainly a lot of activity in the 1950s and 1960s related to joining materials together to form objects. But development of the associated technologies (computers, lasers, controllers, etc.) caught up with the concept in the early 1980s. Interestingly, parallel patents were filed in 1984 in Japan (Murutani), France (Andre et al.) and in the USA (Masters in July and Hull in August). All of these patents described a similar concept of fabricating a 3D object by selectively adding material layer-by-layer. While earlier work in Japan is quite well-documented, proving that this concept could be realized, it was the patent by Charles Hull that is generally recognized as the most influential since it gave rise to
2 Development of Additive Manufacturing Technology
Fig. 2.8 The first AM technology from Hull, who founded 3D Systems (photo courtesy of 3D Systems)
3D Systems. This was the first company to commercialize AM technology with the Stereolithography apparatus (Fig. 2.8). Further patents came along in 1986, resulting in three more companies, Helisys (Laminated Object Manufacturing or LOM), Cubital (with Solid Ground Curing, SGC), and DTM with their Selective Laser Sintering (SLS) process. It is interesting to note neither Helisys nor Cubital exist anymore, and only SLS remains as a commercial process with DTM merging with 3D Systems in 2001. In 1989, Scott Crump patented the Fused Deposition Modeling (FDM) process, forming the Stratasys Company. Also in 1989 a group from MIT patented the 3D Printing (3DP) process. These processes from 1989 are heavily used today, with FDM variants currently being the most successful. Rather than forming a company, the MIT group licensed the 3DP technology to a number of different companies, who applied it in different ways to form the basis for different applications of their AM technology. The most successful of these were Z Corp, which focused mainly on low-cost technology, and ExOne, which focused on powdered metal and sandcasting applications. Inkjet technology has become employed to deposit droplets of material directly onto a substrate, where that material hardens and becomes the part itself rather than just as a binder. Sanders developed this process in 1994, and Objet also used this technique to print photocurable resins in droplet form in 2001. There have been numerous failures and successes in AM history, with the previous paragraphs mentioning only a small number. However, it is hard to know whether a specific technology may have failed because of poor business models or by poor timing rather than having a poor process. Helisys appears to have failed with their LOM machine, but there have been at least five variants from Singapore, China, Japan, Israel, and Ireland. The most recent Mcor process laminates colored sheets together rather than the monochrome paper sheets used in the original LOM
2.11 AM around the World
machine. However, Mcor went into receivership, and their IP was acquired by CleanGreen3D in late 2019. Perhaps this is a better application, and perhaps the technology is in a better position to become successful in the future; however the business track record for LOM-based businesses has been consistently poor. Another example is the defunct Ballistic Particle Manufacturing process, which used a 5-axis mechanism to direct wax droplets onto a substrate. Although no company currently uses such an approach for polymers, similar 5-axis deposition schemes are being used for depositing metal and composites. Another important trend that is impacting the development of AM technology is the expiration of many of the foundational patents for key AM processes. We saw an explosion of MEX vendors systems and systems after the first FDM patents expired in the early 2010s. Initial patents in the stereolithography, laser sintering, and LOM have also expired, which is leading to a proliferation of technologies, processes, machines, companies, and competition worldwide.
2.11 AM around the World As was mentioned, early patents were filed in Europe (France), the USA, and Asia (Japan) almost simultaneously. In early years, most pioneering and commercially successful systems came out of the USA. Companies like Stratasys, 3D Systems, and Z Corp have spearheaded the way forward. These companies have generally strengthened over the years, but most new companies have come from outside the USA. In Europe, the first company with a worldwide impact in AM was EOS, Germany. EOS stopped making SL machines following settlement of disputes with 3D Systems but continues to make PBF systems which use lasers to melt polymers, binder-coated sand, and metals. Companies from elsewhere in Europe are smaller but are competitive in their respective marketplaces. Examples of these companies include Phenix  (now part of 3D Systems), Arcam, Strataconception, SLM Solutions, Trumpf, Additive Industries, and Materialise. The last of these, Materialise from Belgium , has seen considerable success in developing software tools to support AM technology. In the early 1980s and 1990s, a number of Japanese companies focused on AM technology. Large companies like Sony and Kira, who established subsidiaries to build AM technology, also became involved. Much of the Japanese technology was based around the photopolymer curing processes. With 3D Systems dominant in much of the rest of the world, these Japanese companies struggled to find market, and many of them failed to become commercially viable, even though their technology showed some initial promise. Some of this demise may have resulted in the unusually slow uptake of CAD technology within Japanese industry in general. Although the Japanese company CMET  still seems to be doing well, you will likely find more non-Japanese made machines in Japan than home-grown ones. AM technology has also been developed in other parts of Asia, most notably in Korea and China. Korean AM companies have had little international impact; how-
2 Development of Additive Manufacturing Technology
ever, quite a few Chinese manufacturers have been active for a number of years and are beginning to make inroads into markets in Europe and the Americas. Patent conflicts with the earlier US, Japanese, and European designs have meant that many of these machines were not able to be sold outside of China. Earlier Chinese machines were also thought to be of questionable quality, but more recent machines have markedly improved performance (like the machine shown in Fig. 2.9). Chinese machines primarily reflect the SL, FDM, and SLS technologies found elsewhere in the world, and the expiration of initial patents for almost every type of AM technology has created an opening for Chinese companies to compete worldwide. A particular country of interest in terms of AM technology development is Israel. One of the earliest AM machines was developed by the Israeli company Cubital. Although this technology was not a commercial success, in spite of early installations around the world, they demonstrated a number of innovations not found in other machines, including layer processing through a mask, removable secondary support materials and milling after each layer to maintain a constant layer thickness. Some of the concepts used in Cubital can be found in Sanders machines as well as machines from another Israeli company, Objet. Objet joined with Stratasys and moved Stratasy’s headquarters to Israel. The success of Objet’s droplet deposition technology as well as other software and hardware startups in the AM arena makes Israel an outsized player in AM relative to its size.
Fig. 2.9 AM technology from Beijing Yinhua Co. Ltd., China
2.12 AM Standards
2.12 AM Standards Standards in conventional manufacturing play significant roles in helping organizations develop, manufacture, and supply goods and services in a more efficient, effective, and safer manner. Standards in AM can fulfill the same roles. Companies use AM standards to learn to adopt AM technologies, gain confidence in AM usage, communicate with suppliers and customers using a common language, and specify materials and their properties, among others. More specifically, current AM standards assist the specification of types of technical requirements expected when ordering parts, specification of what is needed to qualify a material or process, understanding of how to ensure safe machine operations and environments, and characterization of properties of fabricated parts. In 2009, the authors of this book worked with ASTM International to create the F42 Committee to develop AM standards. Several other standards organizations followed in the next years, including ISO, SAE, and ASME. In 2013, ASTM and ISO formed a partnership to develop and promote AM standards in a landmark agreement between the organizations. The Society of Automotive Engineers (SAE) is developing standards for the aerospace industry for metal AM technologies. The American Society of Mechanical Engineers (ASME) is investigating modifications to their dimensioning and tolerancing standards to accommodate unique characteristics of AM. In 2017, a partnership between the American National Standards Institute (ANSI) and America Makes  released a standardization roadmap that identified 89 gaps, i.e., topics for which standards are needed, and corresponding recommendations ; their second roadmap in 2018 continues to guide standardization efforts worldwide. Within ASTM F42, standards development occurs within six subcommittees on test methods, design, materials and processes, environment health and safety, applications (which has nine sub-subcommittees for various industries), and data. The test methods subcommittee develops new test standards for AM-fabricated specimens and provides guides on how to adopt existing standards to the unique characteristics of AM parts. The design subcommittee develops data exchange standards, including the Additive Manufacturing Format (AMF) ; guides on how to use data exchange formats for multiple materials, medical imaging, etc.; and design for AM guides. In the materials and processes subcommittee, standards are developed for AM-fabricated materials, technical guides for specific processes, finished part properties, post-processing methods, and requirements for purchased AM parts. The last topic is represented by a joint ISO/ASTM standard  that specifies the types of information that suppliers and customers of AM parts should consider to meet acceptance requirements. The environment, health, and safety subcommittee develops standards for operator safety, allowable indoor air quality requirements for AM printers, and related topics. In the applications subcommittee, many standards under development focus on qualification issues that arise in a wide range of industries. Additionally, they have participation from other US federal agencies that oversee specific industries, including the US Food and Drug Administration (FDA) for
2 Development of Additive Manufacturing Technology ISO/ASTM 52900 AM Terminology
ISO/ASTM 52910 General Design Guide ISO/ASTM 52911 PBF Design Guides
ISO/ASTM 52922 DED Design Guide
ISO/ASTM 52915 AMF Format ISO/ASTM 52901 Purchased AM Parts
ISO/ASTM 52912 (TR) Design for functionally Graded Materials
Material Extrusion Design Guide
Design Guide for Post-Processing
F3055 Inconel 718 F3056 Inconel 625
F3049 Characterize Powders
F3184 Stainless Steel UNS S31603
Metal Powder Bed Fusion F3303 Polymer PBF F3091 Directed Energy Deposition F3187
F2971 Reporting data on test specimens F3122 Guide evaluation mechanical properties of metals F3213 Part Properties: Cobalt-28 Chromium-6 Mo F3301 Thermal Post-Processing F3302 Part Properties: Titanium via PBF ISO/ASTM 52902 Test artifacts, geometric capability ISO/ASTM 52921 Terminology for AMCoordinate System
F3318 Aluminum AlSi10 Mg
Fig. 2.10 Current ASTM and ISO standards and their relationships
edical devices and the Federal Aviation Administration (FAA) for aerospace m applications. A snapshot of ASTM and ISO standards available in 2020 is shown in Fig. 2.10, arranged according to the product development stage of relevance. The AM terminology standard provides the foundation for the others. The designer receives guidance from the various design guides during the design process and then can rely on the AMF file format to exchange their parts with the manufacturer. For contracting, the purchased AM parts standard provides guidance. Many standards for materials have been developed, with a focus on metals so far, as well as a standard on powder characterization. For AM fabrication, standards support test specimen reporting data, guidance on evaluating mechanical properties, finished part properties, post- processing methods, etc. As mentioned, several organizations are actively developing standards that should impact AM technology and practices. The specifics presented about ASTM and ISO are meant to illustrate some of the current accomplishments and organization of the activity. In the future, a much more comprehensive set of standards will be available to guide the AM field; these standards will be the product of concerted efforts among many professionals in many standards organizations, companies, universities, and government agencies.
2.13 T he Future? Rapid Prototyping Develops into Direct Digital Manufacturing How might the future of AM look? The ability to “grow” parts may form the core to the answer to that question. The true benefit behind AM is the fact that we do not really need to design the part according to how it is to be manufactured. We would prefer to design the part to perform a particular function. Avoiding the need to con-
sider how the part can be manufactured certainly simplifies the process of design and allows the designer to focus more on the intended application. The design flexibility of AM is making this more and more possible. An example of geometric flexibility is customization of a product. If a product is specifically designed to suit the needs of a unique individual, then it can truly be said to be customized. Imagine being able to modify your mobile phone so that it fits snugly into your hand based on the dimensions gathered directly from your hand. Imagine a hearing aid that can fit precisely inside your ear because it was made from an impression of your ear canal (like those shown in Fig. 2.11). Such things are possible using AM because it has the capacity to make one-off parts, directly from digital models that may not only include geometric features but may also include biometric data gathered from a specific individual. With improvements in AM technology, the speed, quality, accuracy, and material properties have all developed to the extent that parts can be made for final use and not just for prototyping. The terms Rapid Manufacturing and Direct Digital Manufacturing (RM and DDM) gained popularity prior to the adoption of the term Additive Manufacturing to represent the use of AM to produce parts which will be used as an end product. Certainly we will continue to use this technology for prototyping for years to come, but we are already entering a time when it is commonplace to manufacture products in low volumes or unique products using AM. We even see these machines being used as home fabrication devices for hobbyists.
2.14 Questions 1. (a) Based upon an Internet search, describe the Solid Ground Curing process developed by Cubital. (b) Solid Ground Curing has been described as a 2D channel (layer) technique. Could it also be described in another category? Why? 2. Make a list of five different metal AM technologies that are currently available on the market today. How can you distinguish between the different systems? What different materials can be processed in these machines? 3. NC machining is often referred to as a 2.5D process. What does this mean? Why might it not be regarded as fully 3D?
Fig. 2.11 RM of custom hearing aids, from a wax ear impression, on to the machine to the final product. (Photo courtesy of EnvisionTEC and Sonova) [47, 48]
2 Development of Additive Manufacturing Technology
4. Provide three instances where a layer-based approach has been used in fabrication, other than AM. 5. Find five countries not specifically mentioned in this chapter where AM technology has been developed commercially and describe the machines. 6. Home fabrication using AM was an area of extensive market speculation in the late 2010s. But adoption of AM as a home fabrication method remains very low as of 2020. Why do you think this is? Do you see a large future opportunity for home fabrication, or do you think it will stay a niche, hobbyist market? Why or why not? 7. How might the future of Additive Manufacturing (AM) look? Give one specific example of geometric flexibility as a customization of a product. 8. Which of the Additive Manufacturing processes do you believe to be most suitable for home/domestic use and why? 9. What are four ways AM relies on computers that are different from traditional manufacturing? 10. Briefly describe some of the technologies that have contributed to the advancement of AM techniques. 11. MIT performed a study on using silkworm patterns for distributing silk in 2013 (available http://www.dezeen.com/2013/03/13/mit-researchers-to-3d-print-apavilion-by-imitating-silkworms/). How does this apply to Additive Manufacturing? 12. Find three parts that were created via three differing Additive Manufacturing Technologies. Present the picture of the part, the process used for production, the material used, and what is it about the part that gives an idea of the process used to create it. 13. Describe three Additive Manufacturing process types and attributes. Include example companies, materials utilized in machines, and typical markets. 14. What is the AMF format? What are the differences between the AMF format and an STL file? Compare the AMF format to STL files by describing at least 5 advantages AMF over STL file.
References 1. Zuse Z3 Computer. (2020). http://www.zib.de/zuse 2. Goldstine, H. H., & Goldstine, A. (1946). The electronic numerical integrator and computer (eniac). Mathematical Tables and Other Aids to Computation, 2(15), 97–110. 3. Wilkes, M. V., & Renwick, W. (1949). The EDSAC-an electronic calculating machine. Journal of Scientific Instruments, 26(12), 385. 4. Waterloo Computer Science Club. (2020). Talk by Bill Gates. http://csclub.uwaterloo.ca/media 5. Gatlin, J. (1999). Bill Gates: The Path to the Future. Avon Books. 6. Piegl, L., & Tiller, W. (1997). The NURBS Book (2nd ed.). Berlin: Springer. 7. Jamieson, R., & Hacker, H. (1995). Direct slicing of CAD models for rapid prototyping. Rapid Prototyping Journal, 1(2), 4–12. 8. Roscoe, L. (1988). Stereolithography interface specification. America-3D Systems Inc, 27, 10. 9. Protoform. (2020). Space Puzzle Moulding. http://www.protoform.de 10. HASCO. (2020) Precision for Mouldmaking. https://www.hasco.com/en/ 11. LiD. (2020). Architects. http://www.lid-architecture.net
12. Burns, M. (1993). Automated fabrication: improving productivity in manufacturing. Englewood Cliffs: Prentice Hall. 13. Kruth, J.-P., Leu, M.-C., & Nakagawa, T. (1998). Progress in additive manufacturing and rapid prototyping. CIRP Annals, 47(2), 525–540. 14. Chua, C. K., & Leong, K. F. (1998). Rapid prototyping: principles and applications in manufacturing. New York: Wiley. 15. Chua, C. K., Leong, K. F., & Lim, C. S. (2003). Rapid prototyping: principles and applications. Vol. 1. Singapore: World Scientific. 16. Pham, D. T., & Gault, R. S. (1998). A comparison of rapid prototyping technologies. International Journal of Machine Tools and Manufacture, 38(10–11), 1257–1287. 17. MCor Technologies. (2020). http://www.mcortechnologies.com 18. [email protected] (2020). http://www.fabathome.org 19. RepRap. (2020). http://www.reprap.org 20. Stratasys. (2020), 3D Printing & Additive Manufacturing, Stratasys. https://www.stratasys.com/ 21. Microtec. (2020). http://www.microtec-d.com 22. 3D Systems, Stereolithography and selective laser sintering machines. (2020). http:// www.3dsystems.com 23. EOS. (2020). http://www.eos.info 24. Sachs, E., et al. (1992). Three dimensional printing: Rapid tooling and prototypes directly from a CAD model. Journal of Engineering for Industry, 114(4), 481–488. 25. ZCrop (3D Systems). (2020). http://www.zcorp.com 26. Soligen. (2020). http://www.soligen.com 27. Stratasys. (2020). http://www.stratasys.com 28. Solidscape. (2020). http://www.solid-scape.com 29. Kira. (2020). Solid Center machine. www.kiracorp.co.jp/EG/pro/rp/top.html 30. Groza, J. R., & Shackelford, J. F. (2007). Materials processing handbook. Boca Raton: CRC Press. 31. ASTM International. (2015). ISO/ASTM52900–15, standard terminology for additive manufacturing – general principles – terminology. West Conshohocken: ASTM International. 32. Wu, B., et al. (2018). A review of the wire arc additive manufacturing of metals: Properties, defects and quality improvement. Journal of Manufacturing Processes, 35, 127–139. 33. Atwood, C., et al. Laser engineered net shaping (LENS™): A tool for direct fabrication of metal parts. In International Congress on Applications of Lasers & Electro-Optics. 1998. LIA 34. Optomec, LENS process. (2020). http://www.optomec.com 35. White, D. (2003). Ultrasonic object consolidation. US Patents. 36. Arcam. (2020). Electron Beam Melting. http://www.arcam.com 37. Stratoconception, Thick layer hybrid AM. http://www.stratoconception.com 38. Roland, SRP technology. (2020). http://www.rolanddga.com/solutions/rapidprototyping/ 39. Prinz, F. B., & Weiss, L. E. (1998). Novel applications and implementations of shape deposition manufacturing. Naval Research Reviews, 50, 19–26. 40. Phenix, Metal RP technology (Owned By 3D System). (2020). http://www.phenix-systems.com. 41. Materialise. (2020). AM software systems and service provider. http://www.materialise.com. 42. CMET. (2020). Stereolithography technology. http://www.cmet.co.jp 43. America Makes – National Additive Manufacturing Innovation Institute. (2020). www.americamakes.us 44. America Makes & ANSI Additive Manufacturing Standardization Collaborative, Standardization Roadmap for Additive Manufacturing, Version 2.0. (2018). 45. ASTM International. (2015). ISO/ASTM52915–16 Standard Specification for Additive Manufacturing File Format (AMF) Version 1.2. West Conshohocken: ASTM International. 46. ASTM International. (2016). ISO/ASTM52901–16 standard guide for additive manufacturing – general principles – requirements for purchased AM parts. West Conshohocken: ASTM International. 47. Hearing Aid. (2020). EnvisionTEC. https://envisiontec.com/ 48. 3D printing technology for improved hearing, Sonova. (2020). https://www.sonova.biz/en/ features/3d-printing-technology-improved-hearing
Generalized Additive Manufacturing Process Chain
Abstract Although there are an increasing number of AM technologies and variants, they nearly all use a similar process chain. This eight-step process is introduced in this chapter, which aims to provide a framework for the rest of the book. Later chapters address specific process stages in much more detail, leading to ways of overcoming inherent problems within the AM process chain. Furthermore, we look at some application sectors and discuss how the demands of different industries are driving the development of AM.
3.1 Introduction Every product development process involving an Additive Manufacturing machine requires the operator to go through a set sequence of tasks. Easy-to-use “personal” 3D printing machines emphasize the simplicity of this task sequence. These desktop- sized machines are characterized by their low cost, simplicity of use, and ability to be placed in a home or office environment. The larger and more “industrial” AM machines are more capable of being tuned to suit different user requirements and therefore require more expertise to operate, but with a wider variety of possible results and effects that may be put to good use by an experienced operator. Such machines usually require more careful installation in industrial environments. This chapter will take the reader through the different stages of the process that were described in Chap. 1. Different steps in the process will be described with reference to different processes and machines. The objective is to allow the reader to understand how these machines may differ and also to see how each task works and how it may be exploited to the benefit of higher-quality results. As mentioned before, we will refer to eight key steps in the process sequence: • Conceptualization and CAD • Conversion to STL/AMF © Springer Nature Switzerland AG 2021 I. Gibson et al., Additive Manufacturing Technologies, https://doi.org/10.1007/978-3-030-56127-7_3
• • • • • •
3 Generalized Additive Manufacturing Process Chain
Transfer and manipulation of STL/AMF file on AM machine Machine setup Build Part removal and cleanup Post-processing of part Application
There are other ways to break down this process flow, depending on your perspective and equipment familiarity. For example, if you are a designer, you may see more stages in the early product design aspects. Model makers may see more steps in the post-build part of the process. Different AM technologies handle this process sequence differently, so this chapter will also discuss how choice of machine affects the generic process. The use of AM in place of conventional manufacturing processes, such as machining and injection molding, enables designers to ignore some of the constraints of conventional manufacturing. However, conventional manufacturing will remain core to how many products are manufactured. Thus, we must also understand how conventional technologies, such as machining, integrate with AM. This may be particularly relevant to the increasingly popular metal AM processes. Thus, we will discuss how to deal with metal systems in detail.
3.2 The Eight Steps in Additive Manufacture The abovementioned sequence of steps is generally appropriate to all AM technologies. There will be some variations dependent on which technology is being used and also on the design of the particular part. Some steps can be quite involved for some machines but may be trivial for others.
3.2.1 Step 1: Conceptualization and CAD The first step in any product development process is to come up with an idea for how the product will look and function. Conceptualization, sometimes referred to as ideation, can take many forms, from textual and narrative descriptions to sketches and representative models. If AM is to be used, the product description must be in a digital form that allows a physical model to be made. It may be that AM technology will be used to prototype and not build the final product, but in either case, there are many stages in a product development process where digital models are required. AM technology would not exist if it were not for 3D CAD. Only after we gained the ability to represent solid objects in computers were we able to develop technology to physically reproduce such objects. Initially, this was the principle surrounding CNC machining technology in general. AM can thus be described as a direct or streamlined Computer-Aided Design to Computer-Aided Manufacturing (CAD/
3.2 The Eight Steps in Additive Manufacture
1 CAD 2 STL conversion 3 File transfer to machine 4 Machine setup 5 Build 6 Part removal 7 Post-process 8 Application
Fig. 3.1 The eight stages of the AM process 
CAM) process. Unlike most other CAD/CAM technologies, there is little or no intervention between the design and manufacturing stages for AM. The generic AM process must therefore start with 3D CAD information, as shown in Fig. 3.1. There may be a variety of ways for how the 3D source data can be created. This model description could be generated by a design expert via a user interface, by software as part of an automated optimization algorithm, by 3D scanning of an existing physical part, or by some combination of all of these. Most 3D CAD systems are solid modeling systems with surface modeling components; solid models are often constructed by combining surfaces together or by adding thickness to a surface. In the past, 3D CAD modeling software had difficulty creating fully enclosed solid models, and often models would appear to the casual observer to be enclosed but in fact were not mathematically closed. Such models could result in unpredictable output from AM machines, with different AM technologies treating gaps in different ways. Most modern solid modeling CAD tools can now create files without gaps (e.g., “water tight”), resulting in geometrically unambiguous representations of a part. Most CAD packages treat surfaces as construction tools that are used to act on solid models, and this has the effect of maintaining the integrity of the solid data. Provided it can fit inside the machine, typically any CAD model can be made using AM technology without too many difficulties. However, there still remain some older or poorly developed 3D CAD software that may result in solids that are not fully enclosed and produce unreliable AM output. Problems of this manner are normally
3 Generalized Additive Manufacturing Process Chain
detected once the CAD model has been converted into the STL format for building using AM technology.
3.2.2 Step 2: Conversion to STL/AMF Nearly every AM technology uses the STL file format. The term STL was derived from STereoLithograhy, which was the first commercial AM technology from 3D Systems in the 1990s. Considered a de facto standard, STL is a simple way of describing a CAD model in terms of its geometry alone. It works by removing any construction data, modeling history, etc. and approximating the surfaces of the model with a series of triangular facets. The minimum size of these triangles can be set within most CAD software, and the objective is to ensure the models created do not show any obvious triangles on the surface. The triangle size is in fact calculated in terms of the minimum distance between the plane represented by the triangle and the surface it is supposed to represent. In other words, a basic rule of thumb is to ensure that the minimum triangle offset is smaller than the resolution of the AM machine. The process of converting to STL is automatic within most CAD systems, but there is a possibility of errors occurring during this phase. There have been a number of software tools developed to detect such errors and to rectify them if possible. STL files are an unordered collection of triangle vertices and surface normal vectors. As such, an STL file has no units, color, material, or other feature information. These limitations of an STL file have led to the adoption of a new “AMF” file format. This format is an international ASTM/ISO standard format which extends the STL format to include dimensions, color, material, and many other useful features . Many CAD companies and AM hardware vendors support the AMF standard, offering the capability to write or read AMF files as an alternative to STL or other exchange formats. Thus, although the term STL is used throughout the remainder of this textbook, the AMF file could be simply substituted wherever STL appears, as the AMF format has all of the benefits of the STL file format with fewer limitations. STL file repair software, like the MAGICS software from the Belgian company Materialise , is used when there are problems with the STL file that may prevent the part from being built correctly. With complex geometries, it may be difficult for a human to detect such problems when inspecting the CAD or the subsequently generated STL data. If the errors are small, then they may even go unnoticed until after the part has been built. Such software may therefore be applied as a checking stage to ensure that there are no problems with the STL file data before the build is performed. Since STL is essentially a surface description, the corresponding triangles in the files must be pointing in the correct direction; in other words, the surface normal vector associated with the triangle must indicate which side of the triangle is outside vs. inside the part. The cross-section that corresponds to the part layers of a region near an inverted normal vector may therefore be the inversion of what is desired.
3.2 The Eight Steps in Additive Manufacture
Additionally, complex and highly discontinuous geometry may result in triangle vertices that do not align correctly. This may result in gaps in the surface. Various AM technologies may react to these problems in different ways. Some machines may process the STL data in such a way that the gaps are bridged. This bridge may not represent the desired surface; however, and it may be possible that additional, unwanted material may be included in the part. While most errors can be detected and rectified automatically, there may also be a requirement for manual intervention. Software should therefore highlight the problem, indicating what is thought to be inverted triangles, for instance. Since geometries can become very complex, it may be difficult for the software to establish whether the result is in fact an error or something that was part of the original design intent.
3.2.3 S tep 3: Transfer to AM Machine and STL File Manipulation Once the STL file has been created and repaired, it can be sent directly to the target AM machine. Ideally, it should be possible to press a “print” button, and the machine should build the part straight away. This is not usually the case however, and there may be a number of actions required prior to building the part. The first task would be to verify that the part is correct. AM system software normally has a visualization tool that allows the user to view and manipulate the part. The user may wish to reposition the part or even change the orientation to allow it to be built at a specific location within the machine. It is quite common to build more than one part in an AM machine at a time. This may be multiples of the same part (thus requiring a copy function) or completely different STL files. STL files can be linearly scaled quite easily. Some applications may require the AM part to be slightly larger or slightly smaller than the original to account for process shrinkage or coatings; and so scaling may be required prior to building. Applications may also require that the part be identified in some way and some software tools have been developed to add text and simple features to STL formatted data for this purpose. This would be done in the form of adding 3D embossed characters. More unusual cases may even require segmentation of STL files (e.g., for parts that may be too large) or even merging of multiple STL files. For some AM technologies, supports are required to hold the part, while it is being built. This can be done automatically for certain technologies or may require substantial expert decision making for other technologies and applications. For technologies which require supports, part orientation becomes an important decision at this point as well. It should be noted that not all AM machines will have all the functions mentioned here, but numerous STL file manipulation software tools are available for purchase or, in some cases, for free download to perform these functions prior to sending the file to a machine.
3 Generalized Additive Manufacturing Process Chain
3.2.4 Step 4: Machine Setup All AM machines will have at least some setup parameters that are specific to that machine or process. Some machines are only designed to run a few specific materials and give the user few options to vary layer thickness or other build parameters. These types of machines will have very few setup changes to make from build to build. Other machines are designed to run with a variety of materials and may also have some parameters that require optimization to suit the type of part that is to be built or permit parts to be built quicker but with poorer resolution. Such machines can have numerous setup options available. It is common in the more complex cases to have default settings or save files from previously defined setups to help speed up the machine setup process and to prevent mistakes being made. Normally, an incorrect setup procedure will still result in a part being built. The final quality of that part may, however, be unacceptable. In addition to setting up machine process parameters, most machines must be physically prepared for a build. The operator must check to make sure sufficient build material is loaded into the machine to complete the build. For machines which use powder, the powder is often sifted and subsequently loaded and leveled in the machine as part of the setup operation. For processes which utilize a build plate, the plate must be inserted and leveled with respect to the machine axes. Some of these machine setup operations are automated as part of the start-up of a build, but for most machines these operations are done manually by a trained operator. Other aspects such as the direction of printing and selection of proper process parameters have to be considered by operators. Different printing directions can affect the direction of formation of material microstructure which may change the mechanical properties such as breaking elongation and yield stress. Process parameters are important, and unsuitable selection of process parameters may result in formation of pores, unprocessed regions, material deformation, etc. This in turn may lead to dimensional deviation, low surface quality, delamination, cracks, etc. Scan pattern may also change cooling or curing rate and also affect the mechanical properties of the printed parts. Many manufacturers produce industrial machines with the capability of using multiple print-heads, lasers, and other modules which should be considered in order to provide an optimum process strategy for the part geometry and material to be used.
3.2.5 Step 5: Build Although benefitting from the assistance of computers, the first few stages of the AM process are semiautomated tasks that may require considerable manual control, interaction, and decision-making. Once these steps are completed, the process switches to the computer-controlled building phase. This is where the previously mentioned layer-based manufacturing takes place. All AM machines will have a
3.2 The Eight Steps in Additive Manufacture
similar sequence of layering, including a height-adjustable platform or deposition head, material deposition/spreading mechanisms, and layer cross-section formation. Some machines will combine the material deposition and layer formation simultaneously, while others will separate them. As long as no errors are detected during the build, AM machines will repeat the layering process until the build is complete.
3.2.6 Step 6: Removal and Cleanup Ideally, the output from the AM machine should be ready for use with minimal manual intervention. While sometimes this may be the case, more often than not parts will require a significant amount of post-processing before they are ready for use. In all cases, the part must be either separated from a build platform on which the part was produced or removed from excess build material surrounding the part. Some AM processes use additional material other than that used to make the part itself (secondary support materials). Later chapters describe how various AM processes need these support structures to help keep the part from collapsing or warping during the build process. At this stage, it is not necessary to understand exactly how support structures work, but it is necessary to know that they need to be dealt with. While some processes have been developed to produce easy-to-remove supports, there is often a significant amount of manual work required at this stage. For metal supports, a wire EDM machine, band saw, and/or milling equipment may be required to remove the part from the base plate and the supports from the part. There is a degree of operator skill required in part removal, since mishandling of parts and poor technique can result in damage to the part. Different AM parts have different cleanup requirements, but suffice it to say that all processes have some requirement at this stage. The cleanup stage may also be considered as the initial part of the post- processing stage.
3.2.7 Step 7: Post-processing Post-processing refers to the (usually manual) stages of finishing the parts for application purposes. This may involve abrasive finishing, like polishing and sandpapering, or application of coatings. This stage in the process is very application-specific. Some applications may only require a minimum of post-processing. Other applications may require very careful handling of the parts to maintain good precision and finish. Some post-processing may involve chemical or thermal treatment of the part to achieve final part properties. Different AM processes have different results in terms of accuracy, and thus machining to final dimensions may be required. Some processes produce relatively fragile components that may require the use of infiltration and/or surface coatings to strengthen the final part. As already stated, this is
3 Generalized Additive Manufacturing Process Chain
often a manually intensive task due to the complexity of most AM parts. However, some of the tasks can benefit from the use of power tools, CNC milling, and additional equipment, like polishing tubs or drying and baking ovens.
3.2.8 Step 8: Application Following post-processing, parts are ready for use. It should be noted that, although parts may be made from similar materials to those available from other manufacturing processes (like molding and casting), parts may not behave according to standard material specifications. Some AM processes inherently create parts with small voids trapped inside them, which could be the source for part failure under mechanical stress. In addition, some processes may cause the material to degrade during build or for materials not to bond, link, or crystallize in an optimum way. In almost every case, the properties are anisotropic (different properties in different directions). For most metal AM processes, rapid cooling results in different microstructures than those from conventional manufacturing. As a result, AM-produced parts behave differently than parts made using a more conventional manufacturing approach. This behavior may be better or worse for a particular application, and thus a designer should be aware of these differences and take them into account during the design stage. AM materials and processes are improving rapidly, and thus designers must be aware of recent advancements in materials and processes to best determine how to use AM for their needs.
3.3 Variations from One AM Machine to Another The above generic process steps can be applied to every commercial AM technology. As has been noted, different technologies may require more or less attention for a number of these stages. Here we discuss the implications of these variations, not only from process to process but also in some cases within a specific technology. The nominal layer thickness for most machines is around 0.1 mm. However, it should be noted that this is just a rule of thumb. For example, the layer thickness for some Material Extrusion (MEX) machines is 0.254 mm, whereas layer thicknesses between 0.01 and 0.1 mm are commonly used for Vat Photopolymerization (VPP) processes, and small intricate parts made for investment casting and precision engineering applications may have layer thicknesses of less than 0.01 mm. Many technologies have the capacity to vary the layer thickness. The reasoning is that thicker layer parts are quicker to build but are less precise. This may not be a problem for some applications where it may be more important to make the parts as quickly as possible.
3.3 Variations from One AM Machine to Another
Fine detail in a design may cause problems with some AM technologies, such as wall thickness, particularly if there is no choice but to build the part vertically. This is because even though positioning within the machine may be very precise, there is a finite dimension to the droplet size, laser diameter, or extrusion head that essentially defines the finest detail or thinnest wall that can be fabricated. There are other factors that may not only affect the choice of process but also influence some of the steps in the process chain. In particular, the use of different materials even within the same process may affect the time, resources, and skill required to carry out a stage. For example, the use of water-soluble supports in MEX processes may require specialist equipment but will also provide better finish to parts with less hand finishing required than when using conventional supports. Alternatively, some polymers require special attention, like the use (or avoidance) of particular solvents or infiltration compounds. A number of processes benefit from application of sealants or even infiltration of liquid polymers. These materials must be compatible with the part material both chemically and mechanically. Post- processing that involves heat must include awareness of the heat resistance or melting temperature of the materials involved. Abrasive or machining-based processing must also require knowledge of the mechanical properties of the materials involved. If considerable finishing is required, it may also be necessary to include an allowance in the part geometry, perhaps by using scaling of the STL file or offsetting of the part’s surfaces, so that the part does not become worn away too much. Variations between AM technologies will become clarified further in the following chapters, but a general understanding can be achieved by considering whether the build material is processed as a powder, molten material, solid sheet, vat of liquid photopolymer, or ink-jet deposited photopolymer.
3.3.1 Photopolymer-Based Systems It is quite easy to set up systems which utilize photopolymers as the build material. Photopolymer-based systems, however, require files to be created which represent the support structures. All liquid vat systems must use supports from essentially the same material as that used for the part. For Material Jetting (MJT) systems, it is possible to use a secondary support material from parallel ink-jet print heads so that the supports will come off easier. An advantage of photopolymer systems is that accuracy is generally very good, with thin layers and fine precision where required compared with other systems. Photopolymers have historically had poor material properties when compared with other AM materials; however newer resins have been developed that offer improved temperature resistance, strength, and ductility. The main drawback of photopolymer materials is that degradation can occur quite rapidly if UV protective coatings are not applied.
3 Generalized Additive Manufacturing Process Chain
3.3.2 Powder-Based Systems There is no need to use supports for powder systems which deposit a bed of powder layer-by-layer (with the exception of supports for metal systems, as addressed below). Thus, powder bed-based systems are among the easiest to set up for a simple build. Parts made using Binder Jetting (BJT) into a powder bed can be colored by using colored binder material. If color is used then coding the file may take a longer time, as standard STL data does not include color. There are, however, other file formats based around VRML that allow colored geometries to be built, in addition to AMF. Powder Bed Fusion (PBF) processes have a significant amount of unused powder in every build that has been subjected to some level of thermal history. This thermal history may cause changes in the powder. Thus, a well-designed recycling strategy based upon one of several proven methods can help ensure that the material being used is within appropriate limits to guarantee good builds . It is also important to understand the way powders behave inside a machine. For example, some machines use powder feed chambers at either side of the build platform. The powder at the top of these chambers is likely to be less dense than the powder at the bottom, which will have been compressed under the weight of the powder on top. This in turn may affect the amount of material deposited at each layer and density of the final part built in the machine. For very tall builds, this may be a particular problem that can be solved by carefully compacting the powder in the feed chambers before starting the machine and also by adjusting temperatures and powder feed settings during the build.
3.3.3 Molten Material Systems Systems which melt and deposit material in a molten state require support structures. For droplet-based systems like with the Thermojet process, these supports are automatically generated; but with MEX processes or Directed Energy Deposition (DED) systems, supports can either be generated automatically, or the user can use some flexibility to change how supports are made. With water-soluble supports, it is not too important where the supports go, but with breakaway support systems made from the same material as the build material, it is worthwhile to check where the supports go, as surface damage to the part will occur to some extent where these supports were attached before breaking them away. Also, fill patterns for MEX may require some attention, based upon the design intent. Parts can be easily made using default settings, but there may be some benefit in changing aspects of the build sequence if a part or region of a part requires specific characteristics. For example, there are typically small voids in FDM parts that can be minimized by increasing the amount of material extruded in a particular region. This will minimize voids, but at the expenses of part accuracy. Although wax parts made using MJT are good for reproducing fine features, they are difficult to handle because of their low strength and brittleness. ABS parts made using MEX, on the other hand, are among the
3.4 Metal Systems
strongest AM polymer parts available, but when they are desired as a functional end-use part, this may mean they need substantial finishing compared with other processes as they exhibit lower accuracy than some other AM technologies.
3.3.4 Solid Sheets With Sheet Lamination (SHL) methods where the sheets are first placed and then cut, there is no need for supports. Instead, there is a need to process the waste material in such a way that it can be removed from the part. This is generally a straightforward automated process, but there may be a need for close attention to fine detail within a part. Cleaning up the parts can be the most laborious process, and there is a general need to know exactly what the final part is supposed to look like so that damage is not caused to the part during the waste removal stage. Paper-based systems experience problems with handling if they are not carefully and comprehensively finished using sealants and coatings. For polymer SHL, the parts are typically not as sensitive to damage. For metal SHL processes, typically the sheets are cut first and then stacked to form the 3D shape, and thus support removal becomes unnecessary.
3.4 Metal Systems As previously mentioned, operation of metal-based AM systems is conceptually similar to polymer systems. However, the following points are worth considering.
3.4.1 The Use of Substrates Most metal systems make use of a base platform or substrate onto which parts are built and from which they must be removed using machining, wire cutting, or a similar method. The need to attach the parts to a base platform is mainly because of the high-temperature gradients between the temporarily molten material and its surroundings, resulting in large residual stress upon cooling. If the material is not rigidly attached to a solid platform, then the part warps as it cools, which means further layers of powder or deposited material could not be spread evenly over top. Therefore, even though these processes may build within a powder bed, there is still a need for supports. Heat transfer from the substrate affects solidification from the molten state and therefore the microstructure and mechanical properties of the built part. As shown in Fig. 3.2, the cross-section of this part is smaller where it is attached to the substrate compared to the points which are far from the substrate. In the top region, the heat conduction to the substrate is slower, and thus the cooling rate decreases. This results in grain and crystal lattice size differences in different regions of the part [5, 6].
3 Generalized Additive Manufacturing Process Chain
d β Phase α Phase
Fig. 3.2 (a) LPBF- SLM Ti-6Al-4V samples. (b) Cross-section. (c) Microstructure for close to substrate. (d) Microstructure far from substrate (Elsevier license number 4523990304932) 
Mechanical properties are highly dependent on microstructure, where finer microstructure results in higher tensile strengths, but lower ductility [8, 9]. In addition, due to high cooling rates, some intermetallic phases may appear in AM-produced parts that are not in conventionally produced components, which may significantly affect mechanical properties like elongation before failure .
3.4.2 Energy Density Energy density can be defined as the amount of energy per unit of distance, area, or volume that is input into a part as it is being built. Energy density is key factor which determines localized temperature and the size of the melt pool being formed . The energy density required to melt metals is much higher than for melting polymers. The high temperatures achieved during metal melting may require more stringent heat shielding, insulation, temperature control, and atmospheric control than for polymer systems.
3.4.3 Weight Metal powder systems may process lightweight titanium powders, but they also process high-density tool steels and even gold powders. The powder handling technology must be capable of withstanding the mass of these materials. This means that power requirements for positioning and handling equipment must be quite substan-
3.4 Metal Systems
tial or gear ratios must be high (and corresponding travel speeds lower) to deal with these tasks. Some companies like Trumpf, 3D Systems, Renishaw, and Additive Industries have included automatic powder handling system for individual or multiple machines. These systems aim to enable a homogeneous build process, reduction of operator time, and increased system security and reliability. Furthermore, some of these systems include automatic sifting and recycling of powder resulting in further reduction of manual handling of materials [12–14].
3.4.4 Accuracy Accuracy of produced parts must consider both surface quality and dimensional accuracy. Metal powder systems are generally at least as accurate as polymer powder systems. Surface finish is characteristically grainy, but part density and part accuracy are very good. Surface roughness is on the order of a few tens to a few hundreds of microns depending on the process and can be likened in general appearance to precision casting technology. Some companies like 3D MicroPrint  provide a superior surface finish of